advertisement

Foundations of Materials Science and Engineering Sixth Edition William F. Smith Late Professor Emeritus of Engineering of University of Central Florida Javad Hashemi, Ph.D. Professor of Mechanical Engineering Florida Atlantic University Dr. Francisco Presuel-Moreno Associate Professor of Ocean and Mechanical Engineering Florida Atlantic University FOUNDATIONS OF MATERIALS SCIENCE AND ENGINEERING, SIXTH EDITION Published by McGraw-Hill Education, 2 Penn Plaza, New York, NY 10121. Copyright © 2019 by McGraw-Hill Education. All rights reserved. Printed in the United States of America. Previous editions © 2010, 2006, and 2004. No part of this publication may be reproduced or distributed in any form or by any means, or stored in a database or retrieval system, without the prior written consent of McGraw-Hill Education, including, but not limited to, in any network or other electronic storage or transmission, or broadcast for distance learning. Some ancillaries, including electronic and print components, may not be available to customers outside the United States. This book is printed on acid-free paper. 1 2 3 4 5 6 7 8 9 LCR 21 20 19 18 ISBN 978-1-259-69655-8 MHID 1-259-69655-3 Portfolio Manager: Thomas Scaife Ph.D. Product Developers: Tina Bower Marketing Manager: Shannon O’Donnell Content Project Managers: Jeni McAtee, Rachael Hillebrand Buyer: Laura Fuller Design: Egzon Shaqri Content Licensing Specialists: Lorraine Buczek Cover Image: Florida Atlantic University Compositor: SPi Global All credits appearing on page or at the end of the book are considered to be an extension of the copyright page. Library of Congress Cataloging-in-Publication Data Names: Smith, William F. (William Fortune), 1931- author. | Hashemi, Javad, 1961- author. Title: Foundations of materials science and engineering / William F. Smith, late professor emeritus of engineering of University of Central Florida, Javad Hashemi, Ph.D., professor of mechanical engineering, Florida Atlantic University. Description: Sixth edition. | New York, NY: McGraw-Hill Education, c2019. | Includes answers to chapter exercises. | Includes index. Identifiers: LCCN 2017048596 | ISBN 9781259696558 (alk. paper) Subjects: LCSH: Materials science. | Materials science—Textbooks. | Materials. | Materials—Textbooks. Classification: LCC TA403 .S5955 2019 | DDC 620.1/1—dc23 LC record available at https://lccn.loc.gov/2017048596 The Internet addresses listed in the text were accurate at the time of publication. The inclusion of a website does not indicate an endorsement by the authors or McGraw-Hill Education, and McGraw-Hill Education does not guarantee the accuracy of the information presented at these sites. mheducation.com/highered ABOUT THE AUTHORS is a Professor of Mechanical Engineering at Florida Atlantic University and is currently serving as the chairperson of the department. Javad received his Ph.D. in Mechanical Engineering from Drexel University in 1988. Prior to his tenure at Florida Atlantic University, Javad served as Professor of Mechanical Engineering and Associate Dean of Research for the College of Engineering at Texas Tech University. Over the course of his career, Dr. Hashemi has amassed extensive educational and research background in the areas of materials, mechanics, and biomechanics. Javad Hashemi The late William F. Smith was Professor Emeritus of Engineering in the Mechanical and Aerospace Engineering Department of the University of Central Florida at Orlando, Florida. He was awarded an M.S. degree in metallurgical engineering from Purdue University and a Sc.D. degree in metallurgy from Massachusetts Institute of Technology. Dr. Smith, who was a registered professional engineer in the states of California and Florida, taught undergraduate and graduate materials science and engineering courses and actively wrote textbooks for many years. He was also the author of Structure and Properties of Engineering Alloys, Second Edition (McGraw-Hill, 1993). Dr. Francisco Presuel-Moreno is an Associate Professor of Ocean and Mechanical Engineering at Florida Atlantic University and directs the Marine Materials and Corrosion Lab. Dr. Presuel-Moreno received his Ph.D. in Engineering Science from the University of South Florida. Prior to his tenure at Florida Atlantic University, Dr. Presuel-Moreno did a Postdoctoral stay at the Materials Science and Engineering department at the University of Virginia. Over the course of his career, Dr. Presuel-Moreno has accumulated extensive educational and research background, including marine materials, metallic corrosion in concrete, durability of reinforced concrete structures, non-destructive testing and experimental and computational modeling of corrosion processes. iii TABLE OF CONTENTS Preface xv CHAPTER 1 Introduction to Materials Science and Engineering 2 1.1Materials and Engineering 3 1.2Materials Science and Engineering 7 1.3Types of Materials 9 1.3.1 Metallic Materials 9 1.3.2 Polymeric Materials 11 1.3.3 Ceramic Materials 14 1.3.4 Composite Materials 16 1.3.5 Electronic Materials 18 1.4Competition Among Materials 19 1.5Recent Advances in Materials Science and Technology and Future Trends 21 1.5.1 Smart Materials 21 1.5.2 Nanomaterials 23 1.6Design and Selection 24 1.7Summary 26 1.8Definitions 26 1.9Problems 27 CHAPTER 2 Atomic Structure and Bonding 30 2.1Atomic Structure and Subatomic Particles 31 2.2Atomic Numbers, Mass Numbers, and Atomic Masses 35 2.2.1 Atomic Numbers and Mass Numbers 35 2.3The Electronic Structure of Atoms 39 2.3.1 Planck’s Quantum Theory and Electromagnetic Radiation 39 2.3.2 Bohr’s Theory of the Hydrogen Atom 40 2.3.3 The Uncertainty Principle and Schrödinger’s Wave Functions 44 iv 2.3.4 Quantum Numbers, Energy Levels, and Atomic Orbitals 47 2.3.5 The Energy State of Multielectron Atoms 50 2.3.6 The Quantum-Mechanical Model and the Periodic Table 52 2.4Periodic Variations in Atomic Size, Ionization Energy, and Electron Affinity 55 2.4.1 Trends in Atomic Size 55 2.4.2 Trends in Ionization Energy 56 2.4.3 Trends in Electron Affinity 58 2.4.4 Metals, Metalloids, and Nonmetals 60 2.5Primary Bonds 60 2.5.1 Ionic Bonds 62 2.5.2 Covalent Bonds 68 2.5.3 Metallic Bonds 75 2.5.4 Mixed Bonding 77 2.6Secondary Bonds 79 2.7Summary 82 2.8Definitions 82 2.9Problems 84 CHAPTER 3 Crystal and Amorphous Structure in Materials 92 3.1The Space Lattice and Unit Cells 93 3.2Crystal Systems and Bravais Lattices 94 3.3Principal Metallic Crystal Structures 95 3.3.1 Body-Centered Cubic (BCC) Crystal Structure 97 3.3.2 Face-Centered Cubic (FCC) Crystal Structure 100 3.3.3 Hexagonal Close-Packed (HCP) Crystal Structure 101 3.4Atom Positions in Cubic Unit Cells 104 3.5Directions in Cubic Unit Cells 105 Table of Contents 3.6Miller Indices for Crystallographic Planes in Cubic Unit Cells 109 3.7Crystallographic Planes and Directions in Hexagonal Crystal Structure 114 3.7.1 Indices for Crystal Planes in HCP Unit Cells 114 3.7.2 Direction Indices in HCP Unit Cells 116 3.8Comparison of FCC, HCP, and BCC Crystal Structures 116 3.8.1 FCC and HCP Crystal Structures 116 3.8.2 BCC Crystal Structure 119 3.9Volume, Planar, and Linear Density Unit-Cell Calculations 119 3.9.1 Volume Density 119 3.9.2 Planar Atomic Density 120 3.9.3 Linear Atomic Density and Repeat Distance 122 3.10Polymorphism or Allotropy 123 3.11Crystal Structure Analysis 124 3.11.1 X-Ray Sources 125 3.11.2 X-Ray Diffraction 126 3.11.3 X-Ray Diffraction Analysis of Crystal Structures 128 3.12 Amorphous Materials 134 3.13 Summary 135 3.14 Definitions 136 3.15 Problems 137 CHAPTER 4 Solidification and Crystalline Imperfections 146 4.1Solidification of Metals 147 4.1.1 The Formation of Stable Nuclei in Liquid Metals 149 4.1.2 Growth of Crystals in Liquid Metal and Formation of a Grain Structure 154 4.1.3 Grain Structure of Industrial Castings 155 4.2Solidification of Single Crystals 156 4.3Metallic Solid Solutions 160 4.3.1 Substitutional Solid Solutions 161 4.3.2 Interstitial Solid Solutions 163 4.4 Crystalline Imperfections 165 4.4.1 Point Defects 165 4.4.2 Line Defects (Dislocations) 166 4.4.3 Planar Defects 170 4.4.4 Volume Defects 172 4.5Experimental Techniques for Identification of Microstructure and Defects 173 4.5.1 Optical Metallography, ASTM Grain Size, and Grain Diameter Determination 173 4.5.2 Scanning Electron Microscopy (SEM) 178 4.5.3 Transmission Electron Microscopy (TEM) 179 4.5.4 High-Resolution Transmission Electron Microscopy (HRTEM) 180 4.5.5 Scanning Probe Microscopes and Atomic Resolution 182 4.6 Summary 186 4.7 Definitions 187 4.8 Problems 188 CHAPTER 5 Thermally Activated Processes and Diffusion in Solids 196 5.1Rate Processes in Solids 197 5.2Atomic Diffusion in Solids 201 5.2.1 Diffusion in Solids in General 201 5.2.2 Diffusion Mechanisms 201 5.2.3 Steady-State Diffusion 203 5.2.4 Non–Steady-State Diffusion 206 5.3Industrial Applications of Diffusion Processes 208 5.3.1 Case Hardening of Steel by Gas Carburizing 208 5.3.2 Impurity Diffusion into Silicon Wafers for Integrated Circuits 212 5.4Effect of Temperature on Diffusion in Solids 215 5.5 Summary 218 5.6 Definitions 219 5.7 Problems 219 v vi Table of Contents CHAPTER 6 Mechanical Properties of Metals I 224 6.1The Processing of Metals and Alloys 225 6.1.1 The Casting of Metals and Alloys 225 6.1.2 Hot and Cold Rolling of Metals and Alloys 227 6.1.3 Extrusion of Metals and Alloys 231 6.1.4 Forging 232 6.1.5 Other Metal-Forming Processes 234 6.2Stress and Strain in Metals 235 6.2.1 Elastic and Plastic Deformation 236 6.2.2 Engineering Stress and Engineering Strain 236 6.2.3 Poisson’s Ratio 239 6.2.4 Shear Stress and Shear Strain 240 6.3The Tensile Test and The Engineering Stress-Strain Diagram 241 6.3.1 Mechanical Property Data Obtained from the Tensile Test and the Engineering Stress-Strain Diagram 243 6.3.2 Comparison of Engineering Stress-Strain Curves for Selected Alloys 249 6.3.3 True Stress and True Strain 249 6.4Hardness and Hardness Testing 251 6.5Plastic Deformation of Metal Single Crystals 253 6.5.1 Slipbands and Slip Lines on the Surface of Metal Crystals 253 6.5.2 Plastic Deformation in Metal Crystals by the Slip Mechanism 256 6.5.3 Slip Systems 256 6.5.4 Critical Resolved Shear Stress for Metal Single Crystals 261 6.5.5 Schmid’s Law 261 6.5.6 Twinning 264 6.6Plastic Deformation of Polycrystalline Metals 265 6.6.1 Effect of Grain Boundaries on the Strength of Metals 265 6.6.2 Effect of Plastic Deformation on Grain Shape and Dislocation Arrangements 267 6.6.3 Effect of Cold Plastic Deformation on Increasing the Strength of Metals 270 6.7Solid-Solution Strengthening of Metals 271 6.8Recovery and Recrystallization of Plastically Deformed Metals 272 6.8.1 Structure of a Heavily Cold-Worked Metal before Reheating 273 6.8.2 Recovery 273 6.8.3 Recrystallization 275 6.9Superplasticity in Metals 279 6.10 Nanocrystalline Metals 281 6.11 Summary 282 6.12 Definitions 283 6.13 Problems 285 CHAPTER 7 Mechanical Properties of Metals II 294 7.1Fracture of Metals 295 7.1.1 Ductile Fracture 296 7.1.2 Brittle Fracture 297 7.1.3 Toughness and Impact Testing 300 7.1.4 Ductile-to-Brittle Transition Temperature 302 7.1.5 Fracture Toughness 303 7.2Fatigue of Metals 305 7.2.1 Cyclic Stresses 309 7.2.2 Basic Structural Changes that Occur in a Ductile Metal in the Fatigue Process 310 7.2.3 Some Major Factors that Affect the Fatigue Strength of a Metal 311 7.3Fatigue Crack Propagation Rate 312 7.3.1 Correlation of Fatigue Crack Propagation with Stress and Crack Length 312 7.3.2 Fatigue Crack Growth Rate versus Stress-Intensity Factor Range Plots 314 7.3.3 Fatigue Life Calculations 316 7.4Creep and Stress Rupture of Metals 318 7.4.1 Creep of Metals 318 Table of Contents 7.4.2 The Creep Test 320 7.4.3 Creep-Rupture Test 321 7.5Graphical Representation of Creep- and Stress-Rupture Time-Temperature Data Using the Larsen-Miller Parameter 322 7.6A Case Study In Failure of Metallic Components 324 7.7Recent Advances and Future Directions in Improving The Mechanical Performance of Metals 327 7.7.1 Improving Ductility and Strength Simultaneously 327 7.7.2 Fatigue Behavior in Nanocrystalline Metals 329 7.8Summary 329 7.9Definitions 330 7.10Problems 331 CHAPTER 8 Phase Diagrams 336 8.1Phase Diagrams of Pure Substances 337 8.2Gibbs Phase Rule 339 8.3Cooling Curves 340 8.4Binary Isomorphous Alloy Systems 342 8.5The Lever Rule 344 8.6Nonequilibrium Solidification of Alloys 348 8.7Binary Eutectic Alloy Systems 351 8.8Binary Peritectic Alloy Systems 359 8.9Binary Monotectic Systems 364 8.10Invariant Reactions 365 8.11Phase Diagrams with Intermediate Phases and Compounds 367 8.12Ternary Phase Diagrams 371 8.13Summary 374 8.14Definitions 375 8.15Problems 377 CHAPTER vii 9 Engineering Alloys 388 9.1Production of Iron and Steel 389 9.1.1 Production of Pig Iron in a Blast Furnace 390 9.1.2 Steelmaking and Processing of Major Steel Product Forms 391 9.2The Iron-Carbon System 393 9.2.1 The Iron–Iron-Carbide Phase Diagram 393 9.2.2 Solid Phases in the Fe–Fe3C Phase Diagram 393 9.2.3 Invariant Reactions in the Fe–Fe3C Phase Diagram 394 9.2.4 Slow Cooling of Plain-Carbon Steels 396 9.3Heat Treatment of Plain-Carbon Steels 403 9.3.1 Martensite 403 9.3.2 Isothermal Decomposition of Austenite 408 9.3.3 Continuous-Cooling Transformation Diagram for a Eutectoid Plain-Carbon Steel 413 9.3.4 Annealing and Normalizing of PlainCarbon Steels 415 9.3.5 Tempering of Plain-Carbon Steels 417 9.3.6 Classification of Plain-Carbon Steels and Typical Mechanical Properties 421 9.4Low-Alloy Steels 423 9.4.1 Classification of Alloy Steels 423 9.4.2 Distribution of Alloying Elements in Alloy Steels 423 9.4.3 Effects of Alloying Elements on the Eutectoid Temperature of Steels 424 9.4.4 Hardenability 426 9.4.5 Typical Mechanical Properties and Applications for Low-Alloy Steels 430 9.5Aluminum Alloys 432 9.5.1 Precipitation Strengthening (Hardening) 432 viii Table of Contents 9.5.2 General Properties of Aluminum and Its Production 438 9.5.3 Wrought Aluminum Alloys 440 9.5.4 Aluminum Casting Alloys 444 9.6 Copper Alloys 446 9.6.1 General Properties of Copper 446 9.6.2 Production of Copper 446 9.6.3 Classification of Copper Alloys 446 9.6.4 Wrought Copper Alloys 447 9.7 Stainless Steels 452 9.7.1 Ferritic Stainless Steels 452 9.7.2 Martensitic Stainless Steels 453 9.7.3 Austenitic Stainless Steels 455 9.8 Cast Irons 457 9.8.1 General Properties 457 9.8.2 Types of Cast Irons 457 9.8.3 White Cast Iron 459 9.8.4 Gray Cast Iron 459 9.8.5 Ductile Cast Irons 460 9.8.6 Malleable Cast Irons 462 9.9Magnesium, Titanium, and Nickel Alloys 464 9.9.1 Magnesium Alloys 464 9.9.2 Titanium Alloys 466 9.9.3 Nickel Alloys 468 9.10Special-Purpose Alloys and Applications 468 9.10.1 Intermetallics 468 9.10.2 Shape-Memory Alloys 470 9.10.3 Amorphous Metals 474 9.11 Summary 475 9.12 Definitions 476 9.13 Problems 478 CHAPTER 10 Polymeric Materials 488 10.1 Introduction 489 10.1.1 Thermoplastics 490 10.1.2 Thermosetting Plastics (Thermosets) 490 10.2 Polymerization Reactions 491 10.2.1 Covalent Bonding Structure of an Ethylene Molecule 491 10.2.2 Covalent Bonding Structure of an Activated Ethylene Molecule 492 10.2.3 General Reaction for the Polymerization of Polyethylene and the Degree of Polymerization 493 10.2.4 Chain Polymerization Steps 493 10.2.5 Average Molecular Weight for Thermoplastics 495 10.2.6 Functionality of a Monomer 496 10.2.7 Structure of Noncrystalline Linear Polymers 496 10.2.8 Vinyl and Vinylidene Polymers 498 10.2.9 Homopolymers and Copolymers 499 10.2.10 Other Methods of Polymerization 502 10.3Industrial Polymerization Methods 504 10.4Glass Transition Temperature and Crystallinity in Thermoplastics 506 10.4.1 Glass Transition Temperature 506 10.4.2 Solidification of Noncrystalline Thermoplastics 506 10.4.3 Solidification of Partly Crystalline Thermoplastics 507 10.4.4 Structure of Partly Crystalline Thermoplastic Materials 508 10.4.5 Stereoisomerism in Thermoplastics 510 10.4.6 Ziegler and Natta Catalysts 510 10.5Processing of Plastic Materials 512 10.5.1 Processes Used for Thermoplastic Materials 512 10.5.2 Processes Used for Thermosetting Materials 516 10.6 General-Purpose Thermoplastics 518 10.6.1 Polyethylene 520 10.6.2 Polyvinyl Chloride and Copolymers 523 10.6.3 Polypropylene 525 10.6.4 Polystyrene 525 10.6.5 Polyacrylonitrile 526 10.6.6 Styrene–Acrylonitrile (SAN) 527 10.6.7 ABS 527 10.6.8 Polymethyl Methacrylate (PMMA) 529 10.6.9 Fluoroplastics 530 Table of Contents 10.7 Engineering Thermoplastics 531 10.7.1 Polyamides (Nylons) 532 10.7.2 Polycarbonate 535 10.7.3 Phenylene Oxide–Based Resins 536 10.7.4 Acetals 537 10.7.5 Thermoplastic Polyesters 538 10.7.6 Polyphenylene Sulfide 539 10.7.7 Polyetherimide 540 10.7.8 Polymer Alloys 540 10.8Thermosetting Plastics (Thermosets) 541 10.8.1 Phenolics 543 10.8.2 Epoxy Resins 544 10.8.3 Unsaturated Polyesters 546 10.8.4 Amino Resins (Ureas and Melamines) 547 10.9 Elastomers (Rubbers) 549 10.9.1 Natural Rubber 549 10.9.2 Synthetic Rubbers 553 10.9.3 Properties of Polychloroprene Elastomers 554 10.9.4 Vulcanization of Polychloroprene Elastomers 555 10.10Deformation and Strengthening of Plastic Materials 557 10.10.1 Deformation Mechanisms for Thermoplastics 557 10.10.2 Strengthening of Thermoplastics 559 10.10.3 Strengthening of Thermosetting Plastics 562 10.10.4 Effect of Temperature on the Strength of Plastic Materials 563 10.11Creep and Fracture of Polymeric Materials 564 10.11.1 Creep of Polymeric Materials 564 10.11.2 Stress Relaxation of Polymeric Materials 566 10.11.3 Fracture of Polymeric Materials 567 10.12 Summary 570 10.13 Definitions 571 10.14 Problems 574 CHAPTER ix 11 Ceramics 584 11.1 Introduction 585 11.2Simple Ceramic Crystal Structures 587 11.2.1 Ionic and Covalent Bonding in Simple Ceramic Compounds 587 11.2.2 Simple Ionic Arrangements Found in Ionically Bonded Solids 588 11.2.3 Cesium Chloride (CsCl) Crystal Structure 591 11.2.4 Sodium Chloride (NaCl) Crystal Structure 592 11.2.5 Interstitial Sites in FCC and HCP Crystal Lattices 596 11.2.6 Zinc Blende (ZnS) Crystal Structure 598 11.2.7 Calcium Fluoride (CaF2) Crystal Structure 600 11.2.8 Antifluorite Crystal Structure 602 11.2.9 Corundum (Al2O3) Crystal Structure 602 11.2.10 Spinel (MgAl2O4) Crystal Structure 602 11.2.11 Perovskite (CaTiO3) Crystal Structure 603 11.2.12 Carbon and Its Allotropes 603 11.3 Silicate Structures 607 11.3.1 Basic Structural Unit of the Silicate Structures 607 11.3.2 Island, Chain, and Ring Structures of Silicates 607 11.3.3 Sheet Structures of Silicates 607 11.3.4 Silicate Networks 608 11.4Processing of Ceramics 610 11.4.1 Materials Preparation 611 11.4.2 Forming 611 11.4.3 Thermal Treatments 615 11.5Traditional and Structural Ceramics 618 11.5.1 Traditional Ceramics 618 11.5.2 Structural Ceramics 620 11.6Mechanical Properties of Ceramics 622 11.6.1 General 622 11.6.2 Mechanisms for the Deformation of Ceramic Materials 622 x Table of Contents 11.6.3 Factors Affecting the Strength of Ceramic Materials 624 11.6.4 Toughness of Ceramic Materials 624 11.6.5 Transformation Toughening of Partially Stabilized Zirconia (PSZ) 626 11.6.6 Fatigue Failure of Ceramics 628 11.6.7 Ceramic Abrasive Materials 628 11.7Thermal Properties of Ceramics 629 11.7.1 Ceramic Refractory Materials 629 11.7.2 Acidic Refractories 630 11.7.3 Basic Refractories 631 11.7.4 Ceramic Tile Insulation for the Space Shuttle Orbiter 631 11.8 Glasses 633 11.8.1 Definition of a Glass 633 11.8.2 Glass Transition Temperature 633 11.8.3 Structure of Glasses 633 11.8.4 Compositions of Glasses 636 11.8.5 Viscous Deformation of Glasses 636 11.8.6 Forming Methods for Glasses 640 11.8.7 Tempered Glass 641 11.8.8 Chemically Strengthened Glass 642 11.9Ceramic Coatings and Surface Engineering 643 11.9.1 Silicate Glasses 643 11.9.2 Oxides and Carbides 643 11.10Nanotechnology and Ceramics 644 11.11 Summary 646 11.12 Definitions 647 11.13 Problems 648 CHAPTER 12 Composite Materials 656 12.1 Introduction 657 12.1.1 Classification of Composite Materials 657 12.1.2 Advantages and Disadvantages of Composite Materials over Conventional Materials 658 12.2Fibers for Reinforced-Plastic Composite Materials 659 12.2.1 Glass Fibers for Reinforcing Plastic Resins 659 12.2.2 Carbon Fibers for Reinforced Plastics 662 12.2.3 Aramid Fibers for Reinforcing Plastic Resins 664 12.2.4 Comparison of Mechanical Properties of Carbon, Aramid, and Glass Fibers for Reinforced-Plastic Composite Materials 664 12.3Matrix Materials for Composites 666 12.4Fiber-Reinforced Plastic Composite Materials 667 12.4.1 Fiberglass-Reinforced Plastics 667 12.4.2 Carbon Fiber–Reinforced Epoxy Resins 668 12.5Equations for Elastic Modulus of Composite Laminates: Isostrain and Isostress Conditions 670 12.5.1 Isostrain Conditions 670 12.5.2 Isostress Conditions 673 12.6Open-Mold Processes for Fiber-Reinforced Plastic Composite Materials 675 12.6.1 Hand Lay-Up Process 675 12.6.2 Spray Lay-Up Process 676 12.6.3 Vacuum Bag–Autoclave Process 677 12.6.4 Filament-Winding Process 678 12.7Closed-Mold Processes for Fiber-Reinforced Plastic Composite Materials 678 12.7.1 Compression and Injection Molding 678 12.7.2 The Sheet-Molding Compound (SMC) Process 679 12.7.3 Continuous-Pultrusion Process 680 12.8 Concrete 680 12.8.1 Portland Cement 681 12.8.2 Mixing Water for Concrete 684 12.8.3 Aggregates for Concrete 685 12.8.4 Air Entrainment 685 12.8.5 Compressive Strength of Concrete 686 12.8.6 Proportioning of Concrete Mixtures 686 12.8.7 Reinforced and Prestressed Concrete 687 12.8.8 Prestressed Concrete 688 12.9Asphalt and Asphalt Mixes 690 Table of Contents 12.10 Wood 692 12.10.1 Macrostructure of Wood 692 12.10.2 Microstructure of Softwoods 695 12.10.3 Microstructure of Hardwoods 696 12.10.4 Cell-Wall Ultrastructure 697 12.10.5 Properties of Wood 699 12.11 Sandwich Structures 700 12.11.1 Honeycomb Sandwich Structure 702 12.11.2 Cladded Metal Structures 702 12.12Metal-Matrix and Ceramic-Matrix Composites 703 12.12.1 Metal-Matrix Composites (MMCs) 703 12.12.2 Ceramic-Matrix Composites (CMCs) 705 12.12.3 Ceramic Composites and Nanotechnology 710 12.13 Summary 710 12.14 Definitions 711 12.15 Problems 714 CHAPTER 13 Corrosion 720 13.1Corrosion and Its Economical Impact 721 13.2Electrochemical Corrosion of Metals 722 13.2.1 Oxidation-Reduction Reactions 723 13.2.2 Standard Electrode Half-Cell Potentials for Metals 724 13.3 Galvanic Cells 726 13.3.1 Macroscopic Galvanic Cells with Electrolytes That Are One Molar 726 13.3.2 Galvanic Cells with Electrolytes That Are Not One Molar 728 13.3.3 Galvanic Cells with Acid or Alkaline Electrolytes with No Metal Ions Present 730 13.3.4 Microscopic Galvanic Cell Corrosion of Single Electrodes 731 13.3.5 Concentration Galvanic Cells 733 13.3.6 Galvanic Cells Created by Differences in Composition, Structure, and Stress 736 xi 13.4Corrosion Rates (Kinetics) 738 13.4.1 Rate of Uniform Corrosion or Electroplating of a Metal in an Aqueous Solution 738 13.4.2 Corrosion Reactions and Polarization 741 13.4.3 Passivation 745 13.4.4 The Galvanic Series 745 13.5Types of Corrosion 746 13.5.1 Uniform or General Attack Corrosion 746 13.5.2 Galvanic or Two-Metal Corrosion 748 13.5.3 Pitting Corrosion 749 13.5.4 Crevice Corrosion 751 13.5.5 Intergranular Corrosion 753 13.5.6 Stress Corrosion 755 13.5.7 Erosion Corrosion 758 13.5.8 Cavitation Damage 759 13.5.9 Fretting Corrosion 759 13.5.10 Selective Leaching 759 13.5.11 Hydrogen Damage 760 13.6Oxidation of Metals 761 13.6.1 Protective Oxide Films 761 13.6.2 Mechanisms of Oxidation 763 13.6.3 Oxidation Rates (Kinetics) 764 13.7 Corrosion Control 766 13.7.1 Materials Selection 766 13.7.2 Coatings 767 13.7.3 Design 768 13.7.4 Alteration of Environment 769 13.7.5 Cathodic and Anodic Protection 770 13.8 Summary 771 13.9 Definitions 772 13.10 Problems 773 CHAPTER 14 Electrical Properties of Materials 780 14.1Electrical Conduction In Metals 781 14.1.1 The Classic Model for Electrical Conduction in Metals 781 xii Table of Contents 14.1.2 Ohm’s Law 783 14.1.3 Drift Velocity of Electrons in a Conducting Metal 787 14.1.4 Electrical Resistivity of Metals 788 14.2Energy-Band Model for Electrical Conduction 792 14.2.1 Energy-Band Model for Metals 792 14.2.2 Energy-Band Model for Insulators 794 14.3Intrinsic Semiconductors 794 14.3.1 The Mechanism of Electrical Conduction in Intrinsic Semiconductors 794 14.3.2 Electrical Charge Transport in the Crystal Lattice of Pure Silicon 795 14.3.3 Energy-Band Diagram for Intrinsic Elemental Semiconductors 796 14.3.4 Quantitative Relationships for Electrical Conduction in Elemental Intrinsic Semiconductors 797 14.3.5 Effect of Temperature on Intrinsic Semiconductivity 799 14.4Extrinsic Semiconductors 801 14.4.1 n-Type (Negative-Type) Extrinsic Semiconductors 801 14.4.2 p-Type (Positive-Type) Extrinsic Semiconductors 803 14.4.3 Doping of Extrinsic Silicon Semiconductor Material 805 14.4.4 Effect of Doping on Carrier Concentrations in Extrinsic Semiconductors 805 14.4.5 Effect of Total Ionized Impurity Concentration on the Mobility of Charge Carriers in Silicon at Room Temperature 808 14.4.6 Effect of Temperature on the Electrical Conductivity of Extrinsic Semiconductors 809 14.5Semiconductor Devices 811 14.5.1 The pn Junction 812 14.5.2 Some Applications for pn Junction Diodes 815 14.5.3 The Bipolar Junction Transistor 816 14.6Microelectronics 818 14.6.1 Microelectronic Planar Bipolar Transistors 818 14.6.2 Microelectronic Planar Field-Effect Transistors 819 14.6.3 Fabrication of Microelectronic Integrated Circuits 822 14.7Compound Semiconductors 829 14.8Electrical Properties of Ceramics 832 14.8.1 Basic Properties of Dielectrics 832 14.8.2 Ceramic Insulator Materials 834 14.8.3 Ceramic Materials for Capacitors 835 14.8.4 Ceramic Semiconductors 836 14.8.5 Ferroelectric Ceramics 838 14.9Nanoelectronics 841 14.10 Summary 842 14.11Definitions 843 14.12Problems 845 CHAPTER 15 Optical Properties and Superconductive Materials 850 15.1Introduction 851 15.2Light and the Electromagnetic Spectrum 851 15.3Refraction of Light 853 15.3.1 Index of Refraction 853 15.3.2 Snell’s Law of Light Refraction 855 15.4Absorption, Transmission, and Reflection of Light 856 15.4.1 Metals 856 15.4.2 Silicate Glasses 857 15.4.3 Plastics 858 15.4.4 Semiconductors 860 15.5Luminescence 861 15.5.1 Photoluminescence 862 15.5.2 Cathodoluminescence 862 15.6Stimulated Emission of Radiation and Lasers 864 15.6.1 Types of Lasers 866 Table of Contents 15.7Optical Fibers 868 15.7.1 Light Loss in Optical Fibers 868 15.7.2 Single-Mode and Multimode Optical Fibers 869 15.7.3 Fabrication of Optical Fibers 870 15.7.4 Modern Optical-Fiber Communication Systems 872 15.8Superconducting Materials 873 15.8.1 The Superconducting State 873 15.8.2 Magnetic Properties of Superconductors 874 15.8.3 Current Flow and Magnetic Fields in Superconductors 876 15.8.4 High-Current, High-Field Superconductors 877 15.8.5 High Critical Temperature (Tc ) Superconducting Oxides 879 15.9Definitions 881 15.10Problems 882 CHAPTER 16 Magnetic Properties 886 16.1Introduction 887 16.2Magnetic Fields and Quantities 887 16.2.1 Magnetic Fields 887 16.2.2 Magnetic Induction 889 16.2.3 Magnetic Permeability 890 16.2.4 Magnetic Susceptibility 891 16.3Types of Magnetism 892 16.3.1 Diamagnetism 892 16.3.2 Paramagnetism 892 16.3.3 Ferromagnetism 893 16.3.4 Magnetic Moment of a Single Unpaired Atomic Electron 895 16.3.5 Antiferromagnetism 897 16.3.6 Ferrimagnetism 897 16.4Effect of Temperature on Ferromagnetism 897 16.5Ferromagnetic Domains 898 xiii 16.6Types of Energies that Determine the Structure of Ferromagnetic Domains 899 16.6.1 Exchange Energy 900 16.6.2 Magnetostatic Energy 900 16.6.3 Magnetocrystalline Anisotropy Energy 901 16.6.4 Domain Wall Energy 902 16.6.5 Magnetostrictive Energy 903 16.7The Magnetization and Demagnetization of a Ferromagnetic Metal 905 16.8Soft Magnetic Materials 906 16.8.1 Desirable Properties for Soft Magnetic Materials 906 16.8.2 Energy Losses for Soft Magnetic Materials 906 16.8.3 Iron–Silicon Alloys 907 16.8.4 Metallic Glasses 909 16.8.5 Nickel–Iron Alloys 911 16.9Hard Magnetic Materials 912 16.9.1 Properties of Hard Magnetic Materials 912 16.9.2 Alnico Alloys 915 16.9.3 Rare Earth Alloys 917 16.9.4 Neodymium–Iron–Boron Magnetic Alloys 917 16.9.5 Iron–Chromium–Cobalt Magnetic Alloys 918 16.10Ferrites 921 16.10.1 Magnetically Soft Ferrites 921 16.10.2 Magnetically Hard Ferrites 925 16.11Summary 925 16.12Definitions 926 16.13Problems 929 CHAPTER 17 Biological Materials and Biomaterials 934 17.1Introduction 935 17.2Biological Materials: Bone 936 17.2.1 Composition 936 xiv Table of Contents 17.2.2 Macrostructure 936 17.2.3 Mechanical Properties 936 17.2.4 Biomechanics of Bone Fracture 939 17.2.5 Viscoelasticity of Bone 939 17.2.6 Bone Remodeling 940 17.2.7 A Composite Model of Bone 940 17.3Biological Materials: Tendons and Ligaments 942 17.3.1 Macrostructure and Composition 942 17.3.2 Microstructure 942 17.3.3 Mechanical Properties 943 17.3.4 Structure-Property Relationship 945 17.3.5 Constitutive Modeling and Viscoelasticity 946 17.3.6 Ligament and Tendon Injury 948 17.4Biological Material: Articular Cartilage 950 17.4.1 Composition and Macrostructure 950 17.4.2 Microstructure 950 17.4.3 Mechanical Properties 951 17.4.4 Cartilage Degeneration 952 17.5Biomaterials: Metals in Biomedical Applications 952 17.5.1 Stainless Steels 954 17.5.2 Cobalt-Based Alloys 954 17.5.3 Titanium Alloys 955 17.5.4 Some Issues in Orthopedic Application of Metals 957 17.6Polymers in Biomedical Applications 959 17.6.1 Cardiovascular Applications of Polymers 959 17.6.2 Ophthalmic Applications 960 17.6.3 Drug Delivery Systems 962 17.6.4 Suture Materials 962 17.6.5 Orthopedic Applications 962 17.7Ceramics in Biomedical Applications 963 17.7.1 Alumina in Orthopedic Implants 964 17.7.2 Alumina in Dental Implants 965 17.7.3 Ceramic Implants and Tissue Connectivity 966 17.7.4 Nanocrystalline Ceramics 967 17.8Composites in Biomedical Applications 968 17.8.1 Orthopedic Applications 968 17.8.2 Applications in Dentistry 969 17.9Corrosion in Biomaterials 970 17.10Wear in Biomedical Implants 971 17.11Tissue Engineering 975 17.12Summary 976 17.13Definitions 977 17.14Problems 978 APPENDIX I Important Properties of Selected Engineering Materials 983 APPENDIX II Some Properties of Selected Elements 1040 APPENDIX III Ionic Radii of the Elements 1042 APPENDIX IV Glass Transition Temperature and Melting Temperature of Selected Polymers 1044 APPENDIX V Selected Physical Quantities and Their Units 1045 References for Further Study by Chapter 1047 Glossary 1050 Answers 1062 Index 1067 PREFACE T he subject of materials science and engineering is an essential course to engineers and scientists from all disciplines. With advances in science and technology, development of new engineering fields, and changes in the engineering profession, today’s engineer must have a deeper, more diverse, and up-to-date knowledge of materials-related issues. At a minimum, all engineering students must have the basic knowledge of the structure, properties, processing, and performance of various classes of engineering materials. This is a crucial first step in the materials selection decisions in everyday rudimentary engineering problems. A more in-depth understanding of the same topics is necessary for designers of complex systems, forensic (materials failure) analysts, and research and development engineers/ scientists. Accordingly, to prepare materials engineers and scientists of the future, Foundations of Materials Science and Engineering is designed to present diverse topics in the field with appropriate breadth and depth. The strength of the book is in its balanced presentation of concepts in science of materials (basic knowledge) and engineering of materials (applied knowledge). The basic and applied concepts are integrated through concise textual explanations, relevant and stimulating imagery, detailed sample problems, electronic supplements, and homework problems. This textbook is therefore suitable for both an introductory course in materials at the sophomore level and a more advanced (junior/senior level) second course in materials science and engineering. Finally, the sixth edition and its supporting resources are designed to address a variety of student learning styles based on the well-known belief that not all students learn in the same manner and with the same tools. The following improvements have been made to the sixth edition: ■ ■ Chapter 1, Introduction to Materials Science and Engineering, has been updated to reflect the most recent available data on the use of various classes of materials in diverse industries. The use of materials in aerospace and automotive industries is discussed in detail. The historical competition among major classes of materials has been discussed in more detail and updated. All chapters have been reviewed for accuracy of content, images, and tables. New images representing more recent engineering applications have been included in all chapters. Diffusivity data in Chapter 5 has been updated. The mechanical property discussion in Chapter 6 has been expanded to include ­modulus of resilience and toughness. The iron-carbon phase diagram in Chapter 9 has been updated and improved. The concept of glass transition ­temperature has been expanded upon in the discussion of polymers in Chapter 10. The classification of composite materials in Chapter 12 has been expanded and improved. In Chapter 13, the sign convention in reporting the half-cell potentials has been made consistent with IUPAC conventions. The state of the art in microprocessor manufacturing, capability, and design has been updated. xv Rev Confirming Pages xvi Preface ■ The end-of-chapter problems have been classified according to the learning/ understanding level expected from the student by the instructor. The classification is based on Bloom’s Taxonomy and is intended to help students as well as instructors to set goals and standards for learning objectives. The first group in the classification is the Knowledge and Comprehension Problems. These problems will require students to show learning at the most basic level of recall of information and recognition of facts. Most problems ask the students to perform tasks such as define, describe, list, and name. The second group is the Application and Analysis Problems. In this group, students are required to apply the learned knowledge to the solution of a problem, demonstrate a concept, calculate, and analyze. Finally, the third class of problems is called Synthesis and Evaluation Problems. In this class of problems, the students are required to judge, evaluate, design, develop, estimate, assess, and in general synthesize new understanding based on what they have learned from the chapter. It is worth noting that this classification is not indicative of the level of difficulty, but simply different cognitive levels. ■ For most chapters, new problems—mostly in the synthesis and evaluation c­ ategory—have been developed. These problems are intended to make the students think in a more in-depth and reflective manner. This is an important objective of the authors to help instructors to train engineers and scientists who operate at a higher cognitive domain. ■ The instructors’ PowerPoint® lectures have been updated according to the changes made to various chapters. These detailed, yet succinct, PowerPoint ­lectures are highly interactive and contain technical video clips, tutorials for problem solving, and virtual laboratory experiments. The PowerPoint lectures are designed to address a variety of learning styles including innovative, ­analytic, common sense, and dynamic learners. Not only is this a great presentation tool for the instructor, it creates interest in the student to learn the subject more ­effectively. We strongly recommend that the instructors for this course view and test these PowerPoint lecture presentations. This could be especially helpful for new instructors. Additional resources available through the Instructor Resources are interactive quizzing, and step-by-step, real-life processes; animations; and a searchable materials properties database. ACKNOWLEDGMENTS The co-author, Javad Hashemi, would like to dedicate his efforts on this textbook to the eternal-loving memory of his parents Seyed-Hashem and Sedigheh; to his wife, mentor, and friend, Eva; to his sons Evan Darius and Jonathon Cyrus; and last but not least to his siblings (thank you for your ceaseless love and support). smi96553_fm_i-1 xvi 07/02/18 09:40 AM Rev Confirming Pages Preface xvii The authors would like to acknowledge with appreciation the numerous and valuable comments, suggestions, constructive criticisms, and praise from the following evaluators and reviewers: Gerald Bourne Wendy Dannels Donna Ebenstein Francesco Madaro Sam Mil’shtein Morteza Mohssenzadeh Masoud Naghedolfeizi Margaret Pinnell Ranji Vaidyanathan smi96553_fm_i-1 xvii Javad Hashemi 11/15/18 10:48 AM ABOUT THE COVER A race car is an example of a complex mechanical system that utilizes a variety of materials from all five classes in its structure. For instance, for the race car in the image, the body is made of lightweight carbon fiber composites to save weight, the chassis is made of strong and tough steel alloys, the tires are made of durable volcanized rubber, key components in the engine and brake system are either made of or coated with ceramic materials to withstand high temperature, and a variety of sensors as well as the on-board computer system uses electronic materials. The design and selection of materials for the race car is based on many factors including safety, performance, durability, and cost. xviii McGraw-Hill Connect® is a highly reliable, easyto-use homework and learning management solution that utilizes learning science and awardwinning adaptive tools to improve student results. Homework and Adaptive Learning ▪ Connect’s assignments help students contextualize what they’ve learned through application, so they can better understand the material and think critically. ▪ Connect will create a personalized study path customized to individual student needs through SmartBook®. ▪ SmartBook helps students study more efficiently by delivering an interactive reading experience through adaptive highlighting and review. Over 7 billion questions have been answered, making McGraw-Hill Education products more intelligent, reliable, and precise. Using Connect improves retention rates by 19.8 percentage points, passing rates by 12.7 percentage points, and exam scores by 9.1 percentage points. Quality Content and Learning Resources ▪ Connect content is authored by the world’s best subject matter experts, and is available to your class through a simple and intuitive interface. ▪ The Connect eBook makes it easy for students to access their reading material on smartphones and tablets. They can study on the go and don’t need internet access to use the eBook as a reference, with full functionality. ▪ Multimedia content such as videos, simulations, and games drive student engagement and critical thinking skills. 73% of instructors who use Connect require it; instructor satisfaction increases by 28% when Connect is required. ©McGraw-Hill Education Robust Analytics and Reporting ▪ Connect Insight® generates easy-to-read reports on individual students, the class as a whole, and on specific assignments. ▪ The Connect Insight dashboard delivers data on performance, study behavior, and effort. Instructors can quickly identify students who struggle and focus on material that the class has yet to master. ©Hero Images/Getty Images ▪ Connect automatically grades assignments and quizzes, providing easy-to-read reports on individual and class performance. More students earn As and Bs when they use Connect. Trusted Service and Support ▪ Connect integrates with your LMS to provide single sign-on and automatic syncing of grades. Integration with Blackboard®, D2L®, and Canvas also provides automatic syncing of the course calendar and assignment-level linking. ▪ Connect offers comprehensive service, support, and training throughout every phase of your implementation. ▪ If you’re looking for some guidance on how to use Connect, or want to learn tips and tricks from super users, you can find tutorials as you work. Our Digital Faculty Consultants and Student Ambassadors offer insight into how to achieve the results you want with Connect. www.mheducation.com/connect 3 C H A P T E R Crystal and Amorphous Structure in Materials (a) (a) (a) (b) (b) (c) (c) (b) (d (d)) (c) (e) (e) ((a) © McGraw-Hill Education; (b) © Doug Sherman/Geofile; (c) © Zadiraka Evgenii/Shutterstock; (d) © Getty Images/iStockphoto; (e) Source: James St. John) S olids may be categorized broadly into crystalline and amorphous solids. Crystalline solids, due to orderly structure of their atoms, molecules, or ions, possess welldefined shapes. Metals are crystalline and are composed of well-defined crystals or grains. The grains are small and are not clearly observable due to the opaque nature of metals. In minerals, mostly translucent to transparent in nature, the well-defined crystalline shapes are clearly observable. The following images show the crystalline nature of minerals such as (a) celestite (SrSo4) with a sky blue or celestial color, (b) pyrite (FeS2), also called “fool’s gold” due to its brassy yellow color, (c) amethyst (d) (SiO ), a purple variety (e) of quartz, and (d) halite (NaCl), better known as rock salt. 2 In contrast, amorphous solids have poor or no long-range order and do not solidify with the symmetry and regularity of crystalline solids. As an example, the amorphous structure of hyalite opal or glass opal is shown in Figure e. Note the lack of symmetry and of sharp and well-defined crystal edges. ■ 92 L E A R N I N G O B J E C T I V E S By the end of this chapter, students will be able to 1. Describe what crystalline and noncrystalline (amorphous) materials are. 2. Learn how atoms and ions in solids are arranged in space and identify the basic ­building blocks of solids. 3. Describe the difference between atomic s­ tructure and crystal structure for solid material. 4. Distinguish between crystal structure and ­crystal system. 5. Explain why plastics cannot be 100 percent crystalline in structure. 6. Explain polymorphism or allotropy in materials. 7. Compute the densities for metals ­having b­ ody-centered and face-centered cubic structures. 8. Describe how to use the X-ray diffraction method for material characterization. 9. Write the designation for atom position, d­ irection indices, and Miller indices for cubic crystals. Specify what are the three densely packed structures for most metals. Determine Miller-Bravais indices for hexagonal closepacked structure. Be able to draw directions and planes in cubic and hexagonal crystals. 3.1 THE SPACE LATTICE AND UNIT CELLS The physical structure of solid materials of engineering importance depends mainly on the arrangements of the atoms, ions, or molecules that make up the solid and the bonding forces between them. If the atoms or ions of a solid are arranged in a pattern Animation that repeats itself in three dimensions, they form a solid that has long-range order Tutorial (LRO) and is referred to as a crystalline solid or crystalline material. Examples of crystalline materials are metals, alloys, and some ceramic materials. In contrast to crystalline materials, there are some materials whose atoms and ions are not arranged in a long-range, periodic, and repeatable manner and possess only short-range order (SRO). This means that order exists only in the immediate neighborhood of an atom or a molecule. As an example, liquid water has short-range order in its molecules in which one oxygen atom is covalently bonded to two hydrogen atoms. But this order disappears as each molecule is bonded to other molecules through weak secondary bonds in a random manner. Materials with only short-range order are classified as amorphous (without form) or noncrystalline. A more detailed definition and some examples of amorphous materials are given in Section 3.12. Atomic arrangements in crystalline solids can be described by referring the atoms to the points of intersection of a network of lines in three dimensions. Such a network is called a space lattice (Fig. 3.1a), and it can be described as an infinite three-­ dimensional array of points. Each point in the space lattice has identical surroundings. 93 94 CHAPTER 3 Crystal and Amorphous Structure in Materials c β a (a) α b γ (b) Figure 3.1 (a) Space lattice of ideal crystalline solid. (b) Unit cell showing lattice constants. In an ideal crystal, the grouping of lattice points about any given point are identical with the grouping about any other lattice point in the crystal lattice. Each space lattice can thus be described by specifying the atom positions in a repeating unit cell, such as the one heavily outlined in Figure 3.1a. The unit cell may be considered the smallest subdivision of the lattice that maintains the characteristics of the overall crystal. A group of atoms organized in a certain arrangement relative to each other and associated with lattice points constitutes the motif or basis. The crystal structure may then be defined as the collection of lattice and basis. It is important to note that atoms do not necessarily coincide with lattice points. The size and shape of the unit cell can be described by three lattice vectors a, b, and c, originating from one corner of the unit cell (Fig. 3.1b). The axial lengths a, b, and c and the interaxial angles α, β, and γ are the lattice constants of the unit cell. 3.2 CRYSTAL SYSTEMS AND BRAVAIS LATTICES Tutorial By assigning specific values for axial lengths and interaxial angles, unit cells of different types can be constructed. Crystallographers have shown that only seven different types of unit cells are necessary to create all space lattices. These crystal systems are listed in Table 3.1. Many of the seven crystal systems have variations of the basic unit cell. A.J. Bravais1 showed that 14 standard unit cells could describe all possible lattice networks. These Bravais lattices are illustrated in Figure 3.2. There are four basic types of unit cells: (1) simple, (2) body-centered, (3) face-centered, and (4) base-centered. 1 ugust Bravais (1811–1863). French crystallographer who derived the 14 possible arrangements of points A in space. Confirming Pages 3.3 Principal Metallic Crystal Structures 95 Table 3.1 Classification of space lattices by crystal system Crystal System Axial Lengths and Interaxial Angles Space Lattice Cubic Three equal axes at right angles a = b = c, α = β = γ = 90° Tetragonal Three axes at right angles, two equal a = b ≠ c, α = β = γ = 90° Three unequal axes at right angles a ≠ b ≠ c, α = β = γ = 90° Simple cubic Body-centered cubic Face-centered cubic Simple tetragonal Body-centered tetragonal Simple orthorhombic Body-centered orthorhombic Base-centered orthorhombic Face-centered orthorhombic Simple rhombohedral Orthorhombic Rhombohedral Hexagonal Monoclinic Triclinic Three equal axes, equally inclined a = b = c, α = β = γ ≠ 90° Two equal axes at 120°, third axis at right angles a = b ≠ c, α = β = 90°, γ = 120° Three unequal axes, one pair not at right angles a ≠ b ≠ c, α = γ = 90° ≠ b Three unequal axes, unequally inclined and none at right angles a ≠ b ≠ c, α ≠ β ≠ γ ≠ 90° Simple hexagonal Simple monoclinic Base-centered monoclinic Simple triclinic In the cubic system there are three types of unit cells: simple cubic, body-centered cubic, and face-centered cubic. In the orthorhombic system all four types are represented. In the tetragonal system there are only two: simple and body-centered. The face-centered tetragonal unit cell appears to be missing but can be constructed from four body-centered tetragonal unit cells. The monoclinic system has simple and basecentered unit cells, and the rhombohedral, hexagonal, and triclinic systems have only one simple type of unit cell. 3.3 PRINCIPAL METALLIC CRYSTAL STRUCTURES In this chapter, the principal crystal structures of elemental metals will be discussed in detail. Most ionic and covalent materials also possess a crystal structure which will be discussed in detail in Chapter 11. Most elemental metals (about 90%) crystallize upon solidification into three densely packed crystal structures: body-centered cubic (BCC) (Fig. 3.3a), face-­ centered cubic (FCC) (Fig. 3.3b), and hexagonal close-packed (HCP) (Fig. 3.3c). The HCP structure is a denser modification of the simple hexagonal crystal structure shown in Figure 3.2. Most metals crystallize in these dense-packed structures because energy is released as the atoms come closer together and bond more tightly with each other. Thus, the densely packed structures are in lower and more stable energy arrangements. The extremely small size of the unit cells of crystalline metals that are shown in Figure 3.3 should be emphasized. The cube side of the unit cell of body-centered cubic iron, for smi96553_ch03_092-145.indd 95 07/02/18 09:45 AM Confirming Pages 96 CHAPTER 3 Crystal and Amorphous Structure in Materials c c a a c a a a b a a β b c c a a a Tetragonal b c β a a a a b α a a Monoclinic c a Rhombohedral a b a a c c a c a a Cubic a a Hexagonal* β α γ a b b Orthorhombic Triclinic Figure 3.2 Tutorial Animation smi96553_ch03_092-145.indd 96 The 14 Bravais conventional unit cells grouped according to crystal system. The dots indicate lattice points that, when located on faces or at corners, are shared by other identical lattice unit cells. (Source: W.G. Moffatt, G.W. Pearsall, and J. Wulff, The Structure and Properties of Materials, vol. 1: “Structure,” Wiley, 1964, p. 47.) 07/02/18 09:53 AM 3.3 Principal Metallic Crystal Structures (a) (b) 97 (c) Figure 3.3 Principal metal crystal structure and unit cells: (a) body-centered cubic, (b) ­face-centered cubic, (c) hexagonal close-packed crystal structure (the unit cell is shown by solid lines). example, at room temperature is equal to 0.287 × 10−9 m, or 0.287 nanometer (nm).2 Therefore, if unit cells of pure iron are lined up side by side, in 1 mm there will be 1 unit cell 1 mm × _____________________ = 3.48 × 106 unit cells! 0.287 nm × 10−6 mm/nm Let us now examine in detail the arrangement of the atoms in the three principal crystal structure unit cells. Although an approximation, we shall consider atoms in these crystal structures to be hard spheres. The distance between the atoms (interatomic distance) in crystal structures can be determined experimentally by X-ray diffraction analysis.3 For example, the interatomic distance between two neighboring aluminum atoms in a piece of pure aluminum at 20°C is 0.286 nm. The radius of the aluminum atom in the aluminum metal is assumed to be half the interatomic distance, or 0.143 nm. The atomic radii of selected metals are listed in Tables 3.2 to 3.4. 3.3.1 Body-Centered Cubic (BCC) Crystal Structure First, consider the atomic-site unit cell for the BCC crystal structure shown in Figure 3.4a. In this unit cell, the solid spheres represent the centers where atoms are located and clearly indicate their relative positions. If we represent the atoms in this cell as hard spheres, then the unit cell appears as shown in Figure 3.4b. In this unit cell, we see that the central atom is surrounded by eight nearest neighbors and is said to have a coordination number of 8. If we isolate a single hard-sphere unit cell, we obtain the model shown in Figure 3.4c. Each of these cells has the equivalent of two atoms per unit cell. One complete atom is located at the center of the unit cell, and an eighth of a sphere (an 2 3 1 nanometer = 10−9 meter. Some of the principles of X-ray diffraction analysis will be studied in Section 3.11. Animation Tutorial Confirming Pages 98 CHAPTER 3 Crystal and Amorphous Structure in Materials 4R – 3a a 2a (a) (b) (c) 3a = 4R Figure 3.4 BCC unit cells: (a) atomic-site unit cell, (b) hard-sphere unit cell, and (c) isolated unit cell. Figure 3.5 BCC unit cell showing relationship between the lattice constant a and the atomic radius R. Tutorial Animation octant) is located at each corner of the cell, making the equivalent of another atom. Thus, there is a total of 1 (at the center) + 8 × _18 (at the corners ) = 2atoms per unit cell. The atoms in the BCC unit cell contact each other across the cube diagonal, as indicated in Figure 3.5, so the relationship between the length of the cube side a and the atomic radius R is __ 4R __ √3 a = 4 R or a = ___ (3.1) √3 EXAMPLE PROBLEM 3.1 Iron at 20°C is BCC with atoms of atomic radius 0.124 nm. Calculate the lattice constant a for the cube edge of the iron unit cell. ■ Solution From Figure 3.5 it is seen that the atoms in the BCC unit cell touch across the cube diagonals. Thus, if a is the length of the cube edge, then __ √3 a = 4 R (3.1) where R is the radius of the iron atom. Therefore, considering that three significant digits __ should be used in all calculations, the answer will be (use three significant digits for √3 ) 4R a = ___ __ = √3 smi96553_ch03_092-145.indd 98 4(0.124 nm) ___________ __ = 0.287 nm ◂ √3 use three significant digits 07/02/18 09:56 AM 3.3 Principal Metallic Crystal Structures 99 Table 3.2 Selected metals that have the BCC crystal structure at room temperature (20°C) and their lattice constants and atomic radii Metal Lattice Constant a (nm) Atomic Radius R* (nm) 0.289 0.287 0.315 0.533 0.429 0.330 0.316 0.304 0.125 0.124 0.136 0.231 0.186 0.143 0.137 0.132 Chromium Iron Molybdenum Potassium Sodium Tantalum Tungsten Vanadium __ *Calculated from lattice constants by using Eq. (3.1), R = √3 a / 4. If the atoms in the BCC unit cell are considered to be spherical, an atomic packing factor (APF) can be calculated by using the equation volume of atoms in unit cell _______________________ APF = volume of unit cell (3.2) Using this equation, the APF for the BCC unit cell (Fig. 3.4c) is calculated to be 68% (see Example Problem 3.2). That is, 68% of the volume of the BCC unit cell is occupied by atoms and the remaining 32% is empty space. The BCC crystal structure is not a close-packed structure since the atoms could be packed closer together. Many metals such as iron, chromium, tungsten, molybdenum, and vanadium have the BCC crystal structure at room temperature. Table 3.2 lists the lattice constants and atomic radii of selected BCC metals. Calculate the atomic packing factor (APF) for the BCC unit cell, assuming the atoms to be hard spheres. EXAMPLE PROBLEM 3.2 ■ Solution volume of atoms in BCC unit cell ____________________________ APF = volume of BCC unit cell (3.2) Since there are two atoms per BCC unit cell, the volume of atoms in the unit cell of radius R is 4 Vatoms= (2) __ π R3 = 8.373 R3 (3 ) The volume of the BCC unit cell is Vunit cell= a3 Tutorial 100 CHAPTER 3 Crystal and Amorphous Structure in Materials where a is the lattice constant. The relationship between a and R is obtained from Figure 3.5, which shows that the atoms in the BCC unit cell touch each other across the cubic diagonal. Thus, __ 4R __ √3 a = 4 R or a = ___ (3.1) √3 Thus, Vunit cell= a3= 12.32 R3 The atomic packing factor for the BCC unit cell is, therefore, Vatoms/unit cell _______ 8.373 R3 ____________ APF = = = 0.6796 ≈ 0.68 ◂ Vunit cell 12.32 R3 3.3.2 Face-Centered Cubic (FCC) Crystal Structure Consider next the FCC lattice-point unit cell of Figure 3.6a. In this unit cell, there is one lattice point at each corner of the cube and one at the center of each cube face. The hard-sphere model of Figure 3.6b indicates that the atoms in the FCC crystal structure are packed as close together as possible, and are thus called a close-packed structure. The APF for this close-packed structure is 0.74 as compared to 0.68 for the BCC structure, which is not close-packed. The FCC unit cell as shown in Figure 3.6c has the equivalent of four atoms per unit cell. The eight corner octants account for one atom (8 × _18 = 1), and the six halfatoms on the cube faces contribute another three atoms, making a total of four atoms per unit cell. The atoms in the FCC unit cell contact each other across the cubic face diagonal, as indicated in Figure 3.7, so the relationship between the length of the cube side a and the atomic radius R is __ 4R √2 a = 4R or a = ___ __ (3.3) √2 (a) Figure 3.6 (b) (c) FCC unit cells: (a) atomic-site unit cell, (b) hard-sphere unit cell, and (c) isolated unit cell. Confirming Pages 3.3 Principal Metallic Crystal Structures 101 a 4R 2a 2a = 4R Figure 3.7 FCC unit cell showing relationship between the lattice constant a and atomic radius R. Since the atoms touch across the face diagonals, __ √2 a = 4R. Tutorial Animation The APF for the FCC crystal structure is 0.74, which is greater than the 0.68 factor for the BCC structure. The APF of 0.74 is for the closest packing possible of “spherical atoms.” Many metals such as aluminum, copper, lead, nickel, and iron at elevated temperatures (912°C to 1394°C) crystallize with the FCC crystal structure. Table 3.3 lists the lattice constants and atomic radii for some selected FCC metals. 3.3.3 Hexagonal Close-Packed (HCP) Crystal Structure The third common metallic crystal structure is the hexagonal close-packed (HCP) structure shown in Figures 3.8a and b. Metals do not crystallize into the simple hexagonal crystal structure shown in Figure 3.2 because the APF is too low. The atoms can attain a lower energy and a more stable condition by forming the HCP structure of Figure 3.8b. The APF of the HCP crystal structure is 0.74, the same as that for the FCC crystal structure since in both structures the atoms are packed as tightly as Table 3.3 Selected metals that have the FCC crystal structure at room temperature (20°C) and their lattice constants and atomic radii Metal Aluminum Copper Gold Lead Nickel Platinum Silver Lattice Constant a (nm) Atomic Radius R* (nm) 0.405 0.3615 0.408 0.495 0.352 0.393 0.409 0.143 0.128 0.144 0.175 0.125 0.139 0.144 __ Tutorial * Calculated from lattice constants by using Eq. 3.3, R = √2 a / 4. smi96553_ch03_092-145.indd 101 07/02/18 10:01 AM Confirming Pages 102 CHAPTER 3 Crystal and Amorphous Structure in Materials 1 120° 2 Tutorial 2 60° 1 3 c 2 a (a) (b) c 1 a 1 2 (c) Figure 3.8 HCP crystal structure: (a) schematic of the crystal structure, (b) hard-sphere model, and (c) isolated unit cell schematic. (Source: F.M. Miller Chemistry: Structure and Dynamics, McGraw-Hill, 1984, p. 296.) possible. In both the HCP and FCC crystal structures, each atom is surrounded by 12 other atoms, and thus both structures have a coordination number of 12. The differences in the atomic packing in FCC and HCP crystal structures will be discussed in Section 3.8. The isolated HCP unit cell, also called the primitive cell, is shown in Figure 3.8c. The atoms at locations marked “1” on Figure 3.8c contribute _16 of an atom to the unit cell. The atoms at locations marked “2” contribute __ 121 of an atom to the unit cell. Thus, the atoms at the eight corners of the unit cell collectively contribute one 1 atom (4( _16 ) + 4( __ 12 ) = 1). The atom at location “3” is centered inside the unit cell but extends slightly beyond the boundary of the cell. The total number of atoms inside an HCP unit cell is therefore two (one at corners and one at center). In some textbooks the HCP unit cell is represented by Figure 3.8a and is called the “larger cell.” In such a case, one finds six atoms per unit cell. This is mostly for convenience, and the true unit cell is presented in Figure 3.8c by the solid lines. When presenting the topics of crystal directions and planes we will also use the larger cell for convenience, in addition to the primitive cell. The ratio of the height c of the hexagonal prism of the HCP crystal structure to its basal side a is called the c/a ratio (Fig. 3.8a). The c/a ratio for an ideal HCP crystal structure consisting of uniform spheres packed as tightly together as possible is 1.633. Table 3.4 lists some important HCP metals and their c/a ratios. Of the metals listed, cadmium and zinc have c/a ratios higher than the ideal ratio, which indicates that the atoms in these structures are slightly elongated along the c axis of the HCP unit cell. The metals magnesium, cobalt, zirconium, titanium, and beryllium have c/a ratios less than the ideal ratio. Therefore, in these metals, the atoms are slightly compressed in the direction along the c axis. Thus, for the HCP metals listed in Table 3.4, there is a certain amount of deviation from the ideal hard-sphere model. smi96553_ch03_092-145.indd 102 07/02/18 09:58 AM 3.3 Principal Metallic Crystal Structures 103 Table 3.4 Selected metals that have the HCP crystal structure at room temperature (20°C) and their lattice constants, atomic radii, and c/a ratios Lattice Constants (nm) Metal Cadmium Zinc Ideal HCP Magnesium Cobalt Zirconium Titanium Beryllium a c Atomic Radius R (nm) 0.2973 0.2665 0.5618 0.4947 0.149 0.133 0.3209 0.2507 0.3231 0.2950 0.2286 0.5209 0.4069 0.5148 0.4683 0.3584 0.160 0.125 0.160 0.147 0.113 c/a Ratio 1.890 1.856 1.633 1.623 1.623 1.593 1.587 1.568 % Deviation from Ideality +15.7 +13.6 0 −0.66 −0.66 −2.45 −2.81 −3.98 a. Calculate the volume of the zinc crystal structure unit cell by using the following data: pure zinc has the HCP crystal structure with lattice constants a = 0.2665 nm and c = 0.4947 nm. b. Find the volume of the larger cell. ■ Solution The volume of the zinc HCP unit cell can be obtained by determining the area of the base of the unit cell and then multiplying this by its height (Fig. EP3.3). a. The area of the base of the unit cell is area ABDC of Figure EP3.3a and b. This total area consists of the areas of two equilateral triangles of area ABC of Figure EP3.3b. From Figure EP3.3c, Area of triangle ABC = _ 12 (base)( height) 1 = _ 2 ( a) (a sin 60⚬)= _ 12 a2sin 60⚬ From Figure EP3.3b, Total area of HCP base, area ABDC = (2)(_ 12 a2sin 60⚬) = a2sin 60⚬ From Figure EP3.3a, Volume of zinc HCP unit cell = (a2sin 60⚬)(c) = (0.2665 nm)2(0.8660)(0.4947 nm) = 0.03043 nm3 ◂ EXAMPLE PROBLEM 3.3 104 CHAPTER 3 Crystal and Amorphous Structure in Materials E F C c E F G C a D a D G A C h 60° B A (a) 60° A B a B a (b) (c) Figure EP3.3 Diagrams for calculating the volume of an HCP unit cell. (a) HCP unit cell. (b) Base of HCP unit cell. (c) Triangle ABC removed from base of unit cell. b. From Figure EP3.3a, Volume of “large” zinc HCP cell = 3(volume of the unit cell or primitive cell) = 3(0.0304)= 0.09130 nm3 3.4 ATOM POSITIONS IN CUBIC UNIT CELLS To locate atom positions in cubic unit cells, we use rectangular x, y, and z axes. In crystallography, the positive x axis is usually the direction coming out of the paper, the positive y axis is the direction to the right of the paper, and the positive z axis is the direction to the top (Fig. 3.9). Negative directions are opposite to those just described. +z (0, 0, 1) –x z (–1, 0, 0) Tutorial (0, –1, 0) (1, 0, 1) (0, 1, 0) –y (0, 0, 0) (0, 0, 1) +y ( (0, 0, 0) +x (0, 0, –1) –z x (a) Figure 3.9 (1, 1, 1) a (1, 0, 0) (0, 1, 1) 1, 1, 1 2 2 2 ) (0, 1, 0) y (1, 1, 0) (1, 0, 0) (b) (a) Rectangular x, y, and z axes for locating atom positions in cubic unit cells. (b) Atom positions in a BCC unit cell. 3.5 Directions in Cubic Unit Cells 105 Atom positions in unit cells are located by using unit distances along the x, y, and z axes, as indicated in Fig. 3.9a. For example, the position coordinates for the atoms in the BCC unit cell are shown in Fig. 3.9b. The atom positions for the eight corner atoms of the BCC unit cell are (0, 0, 0) (1, 0, 0) (0, 1, 0) (0, 0, 1) (1, 1, 1) (1, 1, 0) (1, 0, 1) (0, 1, 1) The center atom in the BCC unit cell has the position coordinates (_ 21 , _ 21 , _ 21 ). For simplicity, sometimes only two atom positions in the BCC unit cell are specified, which are (0, 0, 0) and (_ 21 , _ 21 , _ 21 ). The remaining atom positions of the BCC unit cell are assumed to be understood. In the same way, the atom positions in the FCC unit cell can be located. 3.5 DIRECTIONS IN CUBIC UNIT CELLS Often it is necessary to refer to specific directions in crystal lattices. This is especially important for metals and alloys with properties that vary with crystallographic orientation. For cubic crystals, the crystallographic direction indices are the vector components of the direction resolved along each of the coordinate axes and reduced to the smallest integers. To diagrammatically indicate a direction in a cubic unit cell, we draw a direction vector from an origin, which is usually a corner of the cubic cell, until it emerges from the cube surface (Fig. 3.10). The position coordinates of the unit cell where the direction vector emerges from the cube surface after being converted to integers are the direction indices. The direction indices are enclosed by square brackets with no separating commas. For example, the position coordinates of the direction vector OR in Figure 3.10a where it emerges from the cube surface are (1, 0, 0), and so the direction indices for the direction vector OR are [100]. The position coordinates of the direction vector OS (Fig. 3.10a) are (1, 1, 0), and so the direction indices for OS are [110]. The position coordinates for the direction vector OT (Fig. 3.10b) are (1, 1, 1), and so the direction indices of OT are [111]. z z z T Origin [100] x R O y S x (a) Figure 3.10 [210] [110] O Some directions in cubic unit cells. O y [111] (b) z M x [1̄1̄0] y x 1 2 (c) N y Note new origin O (d) Tutorial 106 CHAPTER 3 Crystal and Amorphous Structure in Materials The position coordinates of the direction vector OM (Fig. 3.10c) are (1, _ 21 , 0), and since the direction vectors must be integers, these position coordinates must be multiplied by 2 to obtain integers. Thus, the direction indices of OM become 2(1, _12 , 0) = [210] . The position coordinates of the vector ON (Fig. 3.10d) are (−1, −1, 0). A negative direction index is written with a bar over the index. Thus, the direction indices for the vector ON are [¯ 1¯ 0]. Note that to draw the direction ON inside 1 the cube, the origin of the direction vector had to be moved to the front lower-right corner of the unit cube (Fig. 3.10d). Further examples of cubic direction vectors are given in Example Problem 3.4. Often it is useful to determine the angle between two crystal directions. In addition to geometrical analysis, we can use the definitions of dot product to determine the angles between any two direction vectors. Recall from your knowledge of vectors that A · B = ∥ A ∥ ∥ B ∥ cos θ; A = axi + ay j + azk and B = bxi + by j + bzk also, A·B = axbx+ ayby+ azbz (3.4) therefore, axbx+ ayby+ azbz ________________ cos θ = ∥A∥∥B∥ EXAMPLE PROBLEM 3.4 Draw the following direction vectors in cubic unit cells: a. b. c. d. e. f. [100] and [110] [112] [¯ 10] 1 [¯ 2¯ 3 ] 1 Find the angle between [100] and [110] Find the angle between [112] and [¯ 10] 1 ■ Solution a. The position coordinates for the [100] direction are (1, 0, 0) (Fig. EP3.4a). The ­position coordinates for the [110] direction are (1, 1, 0) (Fig. EP3.4a). b. The position coordinates for the [112] direction are obtained by dividing the direction indices by 2 so that they will lie within the unit cube. Thus, they are ( _ 12 , _ 12 , 1) (Fig. EP3.4b). c. The position coordinates for the [¯ 10] direction are (−1, 1, 0) (Fig. EP3.4c). Note 1 that the origin for the direction vector must be moved to the lower-left front corner of the cube. d. The position coordinates for the [¯ 2¯ 3 ] direction are obtained by first dividing all the 1 indices by 3, the largest index. This gives − 1, _ 23 , − _ 13 for the position coordinates of the ¯ ¯ exit point of the direction [3 21 ], which are shown in Figure EP3.4d. 3.5 Directions in Cubic Unit Cells z z 1 2 107 [112] 1 2 O Origin x [100] O y [110] y 1 2 x 1 2 (a) (b) Note new origin z 2 3 z y O [3̄21̄] [1̄10] y x O Note new origin (c) 1– 3 x (d) Figure EP3.4 Direction vectors in cubic unit cells. e. The angle between directions [100] and [110] can be determined using Eq. 3.4 as follows: _________ ∥ A ∥ = √1 2 + 02+ 02 = 1 _________ __ ∥ B ∥ = √12+ 12+ 02 = √2 axbx+ ayby+ azbz ___________________ (1)(1)+ (0)(1)+ (0)(0) __ 1 __ = __ cos θ = ________________ = ∥A∥∥B∥ √2 (1)(√2 ) θ = 45° f. The angle between directions [112] and [¯ 10] can be determined using Eq. 3.4 as 1 follows: _________ __ ∥ A ∥ = √1 2 + 12+ 22 = √6 __________ __ ∥ B ∥ = √− 12+ 12+ 02 = √2 axbx+ ayby+ azbz ___________________ (1)(− 1)+ (1)(1)+ (2)(0) ___ 0 __ __ cos θ = ________________ = = ___ ∥A∥∥B∥ (√6 )(√2) √12 θ = 90° Tutorial 108 CHAPTER 3 Crystal and Amorphous Structure in Materials The letters u, v, and w are used in a general sense for the direction indices in the x, y, and z directions, respectively, and are written as [uvw]. It is also important to note that all parallel direction vectors have the same direction indices. Directions are said to be crystallographically equivalent if the atom spacing along each direction is the same. For example, the following cubic edge directions are crystallographic equivalent directions: [100], [010], [001], [0¯ 0], [00¯ 1 1], [¯ 00]≡ ⟨100⟩ 1 Equivalent directions are called indices of a family or form. The notation ⟨100⟩ is used to indicate cubic edge directions collectively. Other directions of a form are the cubic body diagonals ⟨111⟩ and the cubic face diagonals ⟨110⟩. EXAMPLE PROBLEM 3.5 Determine the direction indices of the cubic direction shown in Figure EP3.5a. ■ Solution Parallel directions have the same direction indices, and so we move the direction vector in a parallel manner until its tail reaches the nearest corner of the cube, still keeping the vector within the cube. Thus, in this case, the upper-left front corner becomes the new origin for the direction vector (Fig. EP3.5b). We can now determine the position coordinates where the direction vector leaves the unit cube. These are x = −1, y = +1, and z = − _ 16 . The ­position coordinates of the direction where it leaves the unit cube are thus ( − 1, +1, − _ 16 ). The direction indices for this direction are, after clearing the fraction 6x, (− 1, +1, − _ 61 ), or [¯ 6¯ 6 ]. 1 New origin z z 1– 6 1– 2 (0, 0, 0) 1– 3 1– 2 Tutorial y x 1– 3 1– 2 y x (a) (b) Figure EP3.5 EXAMPLE PROBLEM 3.6 Determine the direction indices of the cubic direction between the position coordinates (_ 34 , 0, _ 41 ) and ( _ 14 , _ 12 , _ 12 ). ■ Solution First we locate the origin and termination points of the direction vector in a unit cube, as shown in Figure EP3.6. The fraction vector components for this direction are 3.6 Miller Indices for Crystallographic Planes in Cubic Unit Cells 109 3 1 1 x = − __ − __ = − __ (4 4) 2 1 1 y = __ − 0 = __ (2 ) 2 1 1 1 = __ − __ = __ (2 4) 4 Thus, the vector direction has fractional vector components of − __ 2,1 __ 2,1 __ 4.1 . The direction indices will be in the same ratio as their fractional components. By multiplying the fraction vector components by 4, we obtain [¯ 21] for the direction indices of this vector direction. 2 z )14 , 12 , 12) ) 34 , 0, 14) y x Origin for position coordinates Figure EP3.6 3.6 MILLER INDICES FOR CRYSTALLOGRAPHIC PLANES IN CUBIC UNIT CELLS Sometimes it is necessary to refer to specific lattice planes of atoms within a crystal structure, or it may be of interest to know the crystallographic orientation of a plane or group of planes in a crystal lattice. To identify crystal planes in cubic crystal structures, the Miller notation system4 is used. The Miller indices of a crystal plane are defined as the reciprocals of the fractional intercepts (with fractions cleared) that the plane makes with the crystallographic x, y, and z axes of the three nonparallel edges of the cubic unit cell. The cube edges of the unit cell represent unit lengths, and the intercepts of the lattice planes are measured in terms of these unit lengths. The procedure for determining the Miller indices for a cubic crystal plane is as follows: 1. Choose a plane that does not pass through the origin at (0, 0, 0). 2. Determine the intercepts of the plane in terms of the crystallographic x, y, and z axes for a unit cube. These intercepts may be fractions. 4 illiam Hallowes Miller (1801–1880). English crystallographer who published a “Treatise on W Crystallography” in 1839, using crystallographic reference axes that were parallel to the crystal edges and using reciprocal indices. Tutorial Confirming Pages 110 CHAPTER 3 Crystal and Amorphous Structure in Materials 3. Form the reciprocals of these intercepts. 4. Clear fractions and determine the smallest set of whole numbers that are in the same ratio as the intercepts. These whole numbers are the Miller indices of the crystallographic plane and are enclosed in parentheses without the use of commas. The notation (hkl) is used to indicate Miller indices in a general sense, where h, k, and l are the Miller indices of a cubic crystal plane for the x, y, and z axes, respectively. Figure 3.11 shows three of the most important crystallographic planes of cubic crystal structures. Let us first consider the shaded crystal plane in Figure 3.11a, which has the intercepts 1, ∞, ∞ for the x, y, and z axes, respectively. We take the reciprocals of these intercepts to obtain the Miller indices, which are therefore 1, 0, 0. Since these numbers do not involve fractions, the Miller indices for this plane are (100), which is read as the one-zero-zero plane. Next let us consider the second plane shown in Figure 3.11b. The intercepts of this plane are 1, 1, ∞. Since the reciprocals of these numbers are 1, 1, 0, which do not involve fractions, the Miller indices of this plane are (110). Finally, the third plane (Fig. 3.11c) has the intercepts 1, 1, 1, which give the Miller indices (111) for this plane. Consider now the cubic crystal plane shown in Figure 3.12 that has the intercepts _ 13 , _ 23 , 1. The reciprocals of these intercepts are 3 , _ 32 , 1. Since fractional intercepts are not allowed, these fractional intercepts must be multiplied by 2 to clear the _ 32 fraction. Thus, the reciprocal intercepts become 6, 3, 2, and the Miller indices are (632). Further examples of cubic crystal planes are shown in Example Problem 3.7. If the crystal plane being considered passes through the origin so that one or more intercepts are zero, the plane must be moved to an equivalent position in the same unit cell, and the plane must remain parallel to the original plane. This is possible because all equispaced parallel planes are indicated by the same Miller indices. If sets of equivalent lattice planes are related by the symmetry of the crystal system, they are called planes of a family or form, and the indices of one plane of the family are enclosed in braces as {hkl} to represent the indices of a family of symmetrical planes. For example, the Miller indices of the cubic surface planes (100), (010), and (001) are designated collectively as a family or form by the notation {100}. z z z (110) (111) y y (100) y x x (a) x (b) (c) Figure 3.11 Tutorial smi96553_ch03_092-145.indd Miller indices of some important cubic crystal planes: (a) (100), (b) (110), and (c) (111). 110 07/02/18 10:02 AM Confirming Pages 3.6 Miller Indices for Crystallographic Planes in Cubic Unit Cells 111 z (632) O 1 3 y 2 3 x Figure 3.12 Cubic crystal plane (632), which has fractional intercepts. EXAMPLE PROBLEM 3.7 Draw the following crystallographic planes in cubic unit cells: a. b. c. d. (101) (1¯ 0) 1 (221) Draw a (110) plane in a BCC atomic-site unit cell, and list the position coordinates of the atoms whose centers are intersected by this plane. z z (101) Note new origin (11̄0) O O y x x (a) (b) z z (221) (110) O O y x y 1 2 1 2 y x (c) (d ) Figure EP3.7 Various important cubic crystal planes. smi96553_ch03_092-145.indd 111 07/02/18 10:04 AM 112 CHAPTER 3 Crystal and Amorphous Structure in Materials ■ Solution a. First determine the reciprocals of the Miller indices of the (101) plane. These are 1, ∞, 1. The (101) plane must pass through a unit cube at intercepts x = 1 and z = 1 and be parallel to the y axis (Fig. EP3.7a). b. First determine the reciprocals of the Miller indices of the (1¯ 0) plane. These 1 are1, −1, ∞. The (1¯ 0) plane must pass through a unit cube at intercepts x = 1 and 1 y = −1 and be parallel to the z axis. Note that the origin of axes must be moved to the lower-right back side of the cube (Fig. EP3.7b). c. First determine the reciprocals of the Miller indices of the (221) plane. These are _ 21 , _ 21 , 1. The (221) plane must pass through a unit cube at intercepts x = _ 12 , y = _ 12 , and z = 1 (Fig. EP3.7c). d. Atom positions whose centers are intersected by the (110) plane are (1, 0, 0), (0, 1, 0), (1, 0, 1), (0, 1, 1), and ( _2 1 , _2 1 , _2 1 ). These positions are indicated by the solid circles (Fig. EP3.7d). An important relationship for the cubic system, and only the cubic system, is that the direction indices of a direction perpendicular to a crystal plane are the same as the Miller indices of that plane. For example, the [100] direction is perpendicular to the (100) crystal plane. In cubic crystal structures, the interplanar spacing between two closest parallel planes with the same Miller indices is designated dhkl, where h, k, and l are the Miller indices of the planes. This spacing represents the distance from a selected origin containing one plane and another parallel plane with the same indices that is closest to it. For example, the distance between (110) planes 1 and 2, d110, in Figure 3.13 is AB. (110) plane 1 (110) plane 2 A y O B d110 a (110) plane 3 a C x d110 Figure 3.13 Top view of cubic unit cell showing the distance between (110) crystal planes, d110. 3.6 Miller Indices for Crystallographic Planes in Cubic Unit Cells 113 Also, the distance between (110) planes 2 and 3 is d110 and is length BC in Figure 3.13. From simple geometry, it can be shown that for cubic crystal structures a dhkl= _________ ________ √h2+ k2+ l2 (3.5) where dhkl = interplanar spacing between parallel closest planes with Miller indices h, k, and l a = lattice constant (edge of unit cube) h, k, l = Miller indices of cubic planes being considered Determine the Miller indices of the cubic crystallographic plane shown in Figure EP3.8a. EXAMPLE PROBLEM 3.8 ■ Solution First, transpose the plane parallel to the z axis _14 unit to the right along the y axis as shown in Figure EP3.8b so that the plane intersects the x axis at a unit distance from the new origin located at the lower-right back corner of the cube. The new intercepts of the transposed plane with the coordinate axes are now (+1, − __ 125 , ∞). Next, we take the reciprocals of these 12 intercepts to give ( 1, − __ 5 , 0). Finally, we clear the __ 125 fraction to obtain (5¯ 120) for the Miller indices of this plane. z ( 23 – z 1 3 1 4 5 ) = 12 New origin y x y x 3 4 (a) (b) Figure EP3.8 Determine the Miller indices of the cubic crystal plane that intersects the position coordinates ( 1, _ 14 , 0), (1, 1, _ 12 ), ( _34 , 1, _ 14 ), and all coordinate axes. ■ Solution First, we locate the three position coordinates as indicated in Figure EP3.9 at A, B, and C. Next, we join A and B, extend AB to D, and then join A and C. Finally, we join A to C to complete plane ACD. The origin for this plane in the cube can be chosen at E, which gives EXAMPLE PROBLEM 3.9 114 CHAPTER 3 Crystal and Amorphous Structure in Materials z Origin for position coordinates x (1, 1, 12 ) A B C ( 34 , 1, 14 ) y ( 12 , 1, 0) D E (origin for plane) (1, 14 , 0) Figure EP3.9 axial intercepts for plane ACD at x = − _ 12 , y = − _ 34 , and z = _12 . The reciprocals of these axial intercepts are − 2, − _ 43 , and 2. Multiplying these intercepts by 3 clears the fraction, giving Miller indices for the plane of (¯ ¯ 6 6). 4 EXAMPLE PROBLEM 3.10 Copper has an FCC crystal structure and a unit cell with a lattice constant of 0.361 nm. What is its interplanar spacing d220? ■ Solution a 0.361 nm _____________ = 0.128 nm ◂ dhkl= _________ ________ = _____________ 2 2 2 √h + k + l √ (2)2+ (2)2+ (0)2 3.7 CRYSTALLOGRAPHIC PLANES AND DIRECTIONS IN HEXAGONAL CRYSTAL STRUCTURE 3.7.1 Indices for Crystal Planes in HCP Unit Cells Crystal planes in HCP unit cells are commonly identified by using four indices instead of three. The HCP crystal plane indices, called Miller-Bravais indices, are denoted by the letters h, k, i, and l and are enclosed in parentheses as (hkil). These four-digit hexagonal indices are based on a coordinate system with four axes, as shown in Figure 3.14 in an HCP unit cell. There are three basal axes, a1, a2, and a3, which make 120° with each other. The fourth axis or c axis is the vertical axis located at the center of the unit cell. The a unit of measurement along the a1, a2, and a3 axes is the distance between the atoms along these axes and is indicated in Figure 3.14. In the discussion of HCP planes and directions, we will use both the “unit cell” and the “larger cell” for the presentation of concepts. The unit of measurement along the c axis is the height of the unit cell. The reciprocals of the intercepts that a crystal plane makes with the a1, a2, Confirming Pages 3.7 Crystallographic Planes and Directions in Hexagonal Crystal Structure 115 +c +a3 –a1 c –a2 +a2 +a1 –c a –a3 Figure 3.14 The four coordinate axes (a1, a2, a3, and c) of the HCP crystal structure. and a3 axes give the h, k, and i indices, while the reciprocal of the intercept with the c axis gives the l index. Basal Planes The basal planes of the HCP unit cell are very important planes for this unit cell and are indicated in Figure 3.15a. Since the basal plane on the top of the HCP unit cell in Figure 3.15a is parallel to the a1, a2, and a3 axes, the intercepts of this plane with these axes will be at infinity. Thus, a1intercept = ∞, a2intercept = ∞, and a3intercept = ∞. The c axis, however, is unity since the top basal plane intersects the c axis at unit distance, cintercept = 1. Taking the reciprocals of these intercepts gives the Miller-Bravais indices for the HCP basal plane. Thus h = 0, k = 0, i = 0, and l = 1. The HCP basal plane is, therefore, a zero-zero-zero-one or (0001) plane. (0001) (11̄00) (101̄0) E G a3 a3 –a1 c –a2 a2 a1 –a3 (a) B (011̄0) C –a1 c –a2 Intercept is –1 Intercept is +1 F A a1 D Intercept is +1 a2 H Intercept is –1 –a3 (b) Figure 3.15 Miller-Bravais indices of hexagonal crystal planes: (a) basal planes and (b) prism planes. smi96553_ch03_092-145.indd 115 07/02/18 10:04 AM 116 CHAPTER 3 Crystal and Amorphous Structure in Materials Prism Planes Using the same method, the intercepts of the front prism plane (ABCD) of Figure 3.15b are a1intercept = +1, a2intercept = ∞, a3intercept = −1, and cintercept = ∞. Taking the reciprocals of these intercepts gives h = 1, k = 0, i = −1, and l = 0, or the (10¯ 10) plane. Similarly, the ABEF prism plane of Figure 3.15b has the indices (1¯ 100) and the DCGH plane the indices (01¯ 10). All HCP prism planes can be identified collectively as the {10¯ 10} family of planes. Sometimes HCP planes are identified only by three indices (hkl) since h + k = −i. However, the (hkil) indices are used more commonly because they reveal the hexagonal symmetry of the HCP unit cell. 3.7.2 Direction Indices in HCP Unit Cells5 Directions in HCP unit cells are also usually indicated by four indices u, v, t, and w enclosed by square brackets as [uvtw]. The u, v, and t indices are lattice vectors in the a1, a2, and a3 directions, respectively (Fig. 3.16), and the w index is a lattice vector in the c direction. To maintain uniformity for both HCP indices for planes and directions, it has been agreed that u + v = −t for directions. Let us now determine the Miller-Bravais hexagonal indices for the directions a1, a2, and a3, which are the positive basal axes of the hexagonal unit cell. The a1 direction indices are given in Figure 3.16a, the a2 direction indices in Figure 3.16b, and the a3 direction indices in Figure 3.16c. If we need to indicate a c direction also for the a3 direction, this is shown in Figure 3.16d. Figure 3.16e summarizes the positive and negative directions on the upper basal plane of the simple hexagonal crystal structure. 3.8 COMPARISON OF FCC, HCP, AND BCC CRYSTAL STRUCTURES 3.8.1 FCC and HCP Crystal Structures As previously pointed out, both the HCP and FCC crystal structures are close-packed structures. That is, their atoms, which are considered approximate “spheres,” are packed together as closely as possible so that an atomic packing factor of 0.74 is attained.6 The (111) planes of the FCC crystal structure shown in Figure 3.17a have a packing arrangement identical to the (0001) planes of the HCP crystal structure shown in Figure 3.17b. However, the three-dimensional FCC and HCP crystal structures are not identical because there is a difference in the stacking arrangement of their atomic planes, which can best be described by considering the stacking of hard spheres ­representing atoms. As a useful analogy, one can imagine the stacking of planes of equal-sized marbles on top of each other, minimizing the space between the marbles. 5 he topic of direction indices for hexagonal unit cells is not normally presented in an introductory course in T materials but is included here for advanced students. 6 As pointed out in Section 3.3, the atoms in the HCP structure deviate to varying degrees from ideality. In some HCP metals, the atoms are elongated along the c axis, and in other cases, they are compressed along the c axis (see Table 3.4). 3.8 Comparison of FCC, HCP, and BCC Crystal Structures +a2 –a1 +a3 –a3 –a2 a1 +a2 –a1 [1̄21̄0] +a3 [21̄1̄0] 117 –a3 –a2 a1 (a) (b) +a2 –a1 [1̄1̄20] [1̄1̄21] c –a3 +a3 [1̄1̄20] +a2 –a1 –a3 [1̄1̄20] a1 (c) [1̄21̄0] [21̄1̄0] –a1 [1̄21̄0] +a3 –a2 +a3 +a1 –a2 –a2 +a2 –a3 +a1 (d) Figure 3.16 (e) Miller-Bravais hexagonal crystal structure direction indices for principal directions: (a) +a1 axis direction on basal plane, (b) +a2 axis direction on basal plane, (c) +a3 direction axis on basal plane, and (d) +a3 direction axis incorporating c axis. (e) Positive and negative Miller-Bravais directions are indicated in simple hexagonal crystal structure on upper basal plane. Consider first a plane of close-packed atoms designated the A plane, as shown in Figure 3.18. Note that there are two different types of empty spaces or voids between the atoms. The voids pointing to the top of the page are designated a voids and those pointing to the bottom of the page, b voids. A second plane of atoms can be placed over the a or b voids, and the same three-dimensional structure will be produced. Let us place plane B over the a voids, as shown in Figure 3.18b. Now if a third plane of atoms is placed over plane B to form a closest-packed structure, it is possible to form two different close-packed structures. One possibility is to place the atoms of the third plane in the b voids of the B plane. Then the atoms of this third plane will lie directly over those of the A plane and thus can be designated another A plane (Fig. 3.18c). If subsequent planes of atoms are placed in this same alternating stacking arrangement, then 118 CHAPTER 3 Crystal and Amorphous Structure in Materials (111) plane (0001) plane (a) (b) Figure 3.17 Comparison of the (a) FCC crystal structure showing a closepacked (111) plane and (b) an HCP crystal structure showing the close-packed (0001) plane. (Source: W.G. Moffatt, G.W. Pearsall, and J. Wulff, The Structure and Properties of Materials, vol. 1: “Structure,” Wiley, 1964, p. 51.) A plane A plane B plane a void b void a void b void (a) (b) A plane A plane A plane B plane C plane B plane (c) (d) Figure 3.18 Animation Formation of the HCP and FCC crystal structures by the stacking of atomic planes. (a) A plane showing the a and b voids. (b) B plane placed in a voids of plane A. (c) Third plane placed in b voids of B plane, making another A plane and forming the HCP crystal structure. (d) Third plane placed in the a voids of B plane, making a new C plane and forming the FCC crystal structure. (Source: Ander, P.; Sonnessa, A.J., Principles of Chemistry, 1st ed.) 3.9 Volume, Planar, and Linear Density Unit-Cell Calculations [11̄1] (100) plane [1̄11] (110) plane a – 2a (a) (b) Figure 3.19 BCC crystal structure showing (a) the (100) plane and (b) a section of the (110) plane. Note that this is not a close-packed structure, but that the diagonals have closepacked directions. (Source: W.G. Moffatt, G.W. Pearsall and J. Wulff, The Structure and Properties of Materials, vol. 1: “Structure,” Wiley, 1964, p. 51.) the stacking sequence of the three-dimensional structure produced can be denoted by ABABAB. . . . Such a stacking sequence leads to the HCP crystal structure (Fig. 3.17b). The second possibility for forming a simple close-packed structure is to place the third plane in the a voids of plane B (Fig. 3.18d). This third plane is designated the C plane since its atoms do not lie directly above those of the B plane or the A plane. The stacking sequence in this close-packed structure is thus designated ABCABCABC. . . and leads to the FCC structure shown in Figure 3.17a. 3.8.2 BCC Crystal Structure The BCC structure is not a close-packed structure and hence does not have closepacked planes like the {111} planes in the FCC structure and the {0001} planes in the HCP structure. The most densely packed planes in the BCC structure are the {110} family of planes, of which the (110) plane is shown in Figure 3.19b. However, the atoms in the BCC structure do have close-packed directions along the cube diagonals, which are the ⟨111⟩ directions. 3.9 VOLUME, PLANAR, AND LINEAR DENSITY UNIT-CELL CALCULATIONS 3.9.1 Volume Density Using the hard-sphere atomic model for the crystal structure unit cell of a metal and a value for the atomic radius of the metal obtained from X-ray diffraction analysis, a value for the volume density of a metal can be obtained by using the equation mass/unit cell ______________ Volume density of metal = ρυ= volume/unit cell (3.6) 119 120 CHAPTER 3 Crystal and Amorphous Structure in Materials In Example Problem 3.11, a value of 8.933 Mg/m3 (8.933 g/cm3) is obtained for the theoretical density of copper. The handbook experimental value for the density of copper is 8.96 Mg/m3 (8.96 g/cm3). The slightly different density of the experimental value could be attributed to various defects, mismatch where grains meet (grain boundaries), and human error. These crystalline defects are discussed in Chapter 4. Another cause of the discrepancy could also be due to the atoms not being perfect spheres. EXAMPLE PROBLEM 3.11 Copper has an FCC crystal structure and an atomic radius of 0.1278 nm. Assuming the atoms to be hard spheres that touch each other along the face diagonals of the FCC unit cell as shown in Figure 3.7, calculate a theoretical value for the density of copper in mega-grams per cubic meter. The atomic mass of copper is 63.54 g/mol. ■ Solution For the FCC unit cell, 1 ¯ 2a = 4R, where a is the lattice constant of the unit cell, and R is the atomic radius of the copper atom. Thus, 4R _____________ (4)(0.1278 nm) __ a = ___ __ = = 0.3615 nm √2 √2 mass/unit cell ______________ Volume density of copper = ρυ= volume/unit cell (3.6) In the FCC unit cell, there are four atoms/unit cell. Each copper atom has a mass of (63.54 g/ mol) (6.02 × 1023 atoms/mol). Thus, the mass m of Cu atoms in the FCC unit cell is 10−6 Mg ( 4 atoms)( 63.54 g/mol) _ ____________________ m = = 4.220 × 10−28 Mg ) g 6.022 × 1023 atoms/mol ( The volume V of the Cu unit cell is 10−9 m V = a3= 0.361 nm × _______ = 4.724 × 10−29m3 ( nm ) 3 Thus, the theoretical density of copper is m 4.220 × 10−28 Mg ρυ= _ = _______________ = 8.933 Mg / m3(8.933 g/cm3)◂ V 4.724 × 10−29m3 3.9.2 Planar Atomic Density Sometimes it is important to determine the atomic densities on various crystal planes. To do this, a quantity called the planar atomic density is calculated by using the relationship equiv. no. of atoms whose centers are intersected by selected area lanar atomic density = ρp= ___________________________________ P selected area (3.8) For convenience, the area of a plane that intersects a unit cell is usually used in these calculations, as shown, for example, in Figure 3.20 for the (110) plane in a BCC unit 3.9 Volume, Planar, and Linear Density Unit-Cell Calculations 121 z (110) a a – 2a y x – 2a (a) (b) Figure 3.20 (a) A BCC atomic-site unit cell showing a shaded (110) plane. (b) Areas of atoms in BCC unit cell cut by the (110) plane. cell. In order for an atom area to be counted in this calculation, the plane of interest must intersect the center of an atom. In Example Problem 3.12, the (110) plane ­intersects the centers of five atoms, but the equivalent of only two atoms is counted since only onequarter of each of the four corner atoms is included in the area inside the unit cell. Calculate the planar atomic density ρp on the (110) plane of the α iron BCC lattice in atoms per square millimeter. The lattice constant of α iron is 0.287 nm. ■ Solution equiv. no. of atoms whose centers are intersected by selected area _____________________________________________________ ρP= selected area (3.7) The equivalent number of atoms intersected by the (110) plane in terms of the surface area inside the BCC unit cell is shown in Figure 3.22 and is 1 1 atom at center + 4 × __ atoms at four corners of plane = 2 atoms 4 The area intersected by the (110) plane inside the unit cell (selected area) is __ __ (√2 a)(a) = √2 a2 Thus, the planar atomic density is 2 atoms 17.2 atoms __ ρP= ___________ = _________ 2 nm2 √2 (0.287 nm ) 17.2 atoms 1012nm2 = _________ × ________ nm2 mm2 = 1.72 × 1013 atoms / mm2 ◂ EXAMPLE PROBLEM 3.12 122 CHAPTER 3 Crystal and Amorphous Structure in Materials 3.9.3 Linear Atomic Density and Repeat Distance Sometimes it is important to determine the atomic densities in various directions in crystal structures. To do this, a quantity called the linear atomic density is calculated by using the relationship no. of atomic diam. intersected by selected length of line in direction of interest ___________________________________ inear atomic density = ρl= L (3.8) selected length of line The distance between two consecutive lattice points along a specific direction is called the repeat distance. Example Problem 3.13 shows how the linear atomic density can be calculated in the [110] direction in a pure copper crystal lattice. EXAMPLE PROBLEM 3.13 Calculate the linear atomic density ρl in the [110] direction in the copper crystal lattice in atoms per millimeter. Copper is FCC and has a lattice constant of 0.361 nm. ■ Solution The atoms whose centers the [110] direction intersects are shown in Figure EP3.13. We shall select__ the length of the line to be the length of the face diagonal of the FCC unit cell, which is √2 a. The number of atomic diameters intersected by this length of line are _ 12 + 1 + _ 12 = 2 atoms. Thus using Eq. 3.8, the linear atomic density is 2 atoms ___________ 2 atoms 3.92 atoms __ = __ ρl= _______ = _________ nm √2 a √2 (0.361 nm) 3.92 atoms 106 nm = _________× ______ nm mm = 3.92 × 106 atoms / mm ◂ z a o x Figure EP3.13 y [110] Diagram for calculating the linear atomic density in the [110] direction in an FCC unit cell. 3.10 Polymorphism or Allotropy 3.10 POLYMORPHISM OR ALLOTROPY Many elements and compounds exist in more than one crystalline form under different conditions of temperature and pressure. This phenomenon is termed polymorphism, or allotropy. Many industrially important metals such as iron, titanium, and cobalt undergo allotropic transformations at elevated temperatures at atmospheric pressure. Table 3.5 lists some selected metals that show allotropic transformations and the structure changes that occur. Iron exists in both BCC and FCC crystal structures over the temperature range from room temperature to its melting point at 1539°C as shown in Figure 3.21. Alpha (α) iron exists from −273°C to 912°C and has the BCC crystal structure. Gamma (γ) Table 3.5 Allotropic crystalline forms of some metals Metal Crystal Structure at Room Temperature Ca Co Hf Fe FCC HCP HCP BCC Li Na Tl Ti Y Zr BCC BCC HCP HCP HCP HCP C 1539 1394 BCC (>447°C) FCC (>427°C) BCC (>1742°C) FCC (912–1394°C) BCC (>1394°C) HCP (<−193°C) HCP (<−233°C) BCC (>234°C) BCC (>883°C) BCC (>1481°C) BCC (>872°C) Liquid iron δ (delta) iron (BCC) γ (gamma) iron (FCC) Temperature 912 α (alpha) iron (BCC) -273 Figure 3.21 At Other Temperatures Allotropic crystalline forms of iron over temperature ranges at atmospheric pressure. 123 124 CHAPTER 3 Crystal and Amorphous Structure in Materials iron exists from 912°C to 1394°C and has the FCC crystal structure. Delta (δ) iron exists from 1394°C to 1539°C which is the melting point of iron. The crystal structure of δ iron is also BCC but with a larger lattice constant than α iron. EXAMPLE PROBLEM 3.14 Calculate the theoretical volume change accompanying a polymorphic transformation in a pure metal from the FCC to BCC crystal structure. Assume the hard-sphere atomic model and that there is no change in atomic volume before and after the transformation. ■ Solution In the FCC crystal structure unit cell, the atoms are in contact along the face diagonal of the unit cell, as shown in Figure 3.7. Hence, __ 4R √2 a = 4R or a = ___ __ √2 (3.3) In the BCC crystal structure unit cell, the atoms are in contact along the body diagonal of the unit cell as shown in Figure 3.5. Hence, __ 4R √3 a = 4R or a = ___ __ √3 (3.1) The volume per atom for the FCC crystal lattice, since it has four atoms per unit cell, is a3 4R 1 VFCC= __ = ____ __ _ = 5.66 R3 4 ( √2 ) ( 4 ) 3 The volume per atom for the BCC crystal lattice, since it has two atoms per unit cell, is a3 4R 1 VBCC= __ = ____ __ _ = 6.16 R3 2 ( √3 ) ( 2 ) 3 The change in volume associated with the transformation from the FCC to BCC crystal structure, assuming no change in atomic radius, is V − VFCC ΔV _____ = __________ BCC VFCC VFCC 6.16 R3− 5.66 R3 ______________ = 1 00 % = +8.83 % ◂ ( ) 5.66 R3 3.11 CRYSTAL STRUCTURE ANALYSIS Our present knowledge of crystal structures has been obtained mainly by X-ray ­diffraction techniques that use X-rays whose wavelength are the same as the distance between crystal lattice planes. However, before discussing the manner in 3.11 Crystal Structure Analysis Copper X-rays Vacuum Tungsten filament Glass Electrons Cooling water To transformer Target Beryllium window X-rays Metal focusing cup Figure 3.22 Schematic diagram of the cross section of a sealed-off filament X-ray tube. (Source: B. D. Cullity, Elements of X-Ray Diffraction 2nd ed., Addison-Wesley, 1978, p. 23.) which X-rays are diffracted in crystals, let us consider how X-rays are produced for experimental purposes. 3.11.1 X-Ray Sources X-rays used for diffraction are electromagnetic waves with wavelengths in the range 0.05 to 0.25 nm (0.5 to 2.5 Å). By comparison, the wavelength of visible light is of the order of 600 nm (6000 Å). In order to produce X-rays for diffraction purposes, a voltage of about 35 kV is necessary and is applied between a cathode and an anode target metal, both of which are contained in a vacuum, as shown in Figure 3.22. When the tungsten filament of the cathode is heated, electrons are released by thermionic emission and accelerated through the vacuum by the large voltage difference between the cathode and anode, thereby gaining kinetic energy. When the electrons strike the target metal (e.g., molybdenum), X-rays are given off. However, most of the kinetic energy (about 98%) is converted into heat, so the target metal must be cooled externally. The X-ray spectrum emitted at 35 kV using a molybdenum target is shown in Figure 3.23. The spectrum shows continuous X-ray radiation in the wavelength range from about 0.2 to 1.4 Å (0.02 to 0.14 nm) and two spikes of characteristic radiation that are designated the Kα and Kβ lines. The wavelengths of the Kα and Kβ lines are characteristic for an element. For molybdenum, the Kα line occurs at a wavelength of about 0.7 Å (0.07 nm). The origin of the characteristic radiation is explained as follows: first, K electrons (electrons in the n = 1 shell) are knocked out of the atom by highly energetic electrons bombarding the target, leaving excited atoms. Next, some electrons in higher shells (that is, n = 2 or 3) drop down to lower energy levels 125 126 CHAPTER 3 Crystal and Amorphous Structure in Materials To 37.2 16 Relative intensity Mo K α Mo K β 12 Ionization Characteristic radiation 8 N Lα 0 0.2 1.0 0.6 Wavelength λ (Å) Energy Continuous radiation 4 X-ray emission spectrum produced when molybdenum metal is used as the target metal in an X-ray tube operating at 35 kV. M n=3 L n=2 K n=1 Kβ Kα 1.4 Figure 3.23 Lβ n=4 Figure 3.24 Energy levels of electrons in molybdenum showing the origin of Kα and Kβ radiation. to replace the lost K electrons, emitting energy of a characteristic wavelength. The ­transition of electrons from the L (n = 2) shell to the K (n = 1) shell creates energy of the wavelength of the Kα line, as indicated in Figure 3.24. 3.11.2 X-Ray Diffraction Since the wavelengths of some X-rays are about equal to the distance between planes of atoms in crystalline solids, reinforced diffraction peaks of radiation of varying intensities can be produced when a beam of X-rays strikes a crystalline solid. However, before considering the application of X-ray diffraction techniques to crystal structure analysis, let us examine the geometric conditions necessary to produce diffracted or reinforced beams of reflected X-rays. Consider a monochromatic (single-wavelength) beam of X-rays to be incident on a crystal, as shown in Figure 3.25. For simplification, let us allow the crystal planes of atomic scattering centers to be replaced by crystal planes that act as mirrors in reflecting the incident X-ray beam. In Figure 3.25, the horizontal lines represent a set of parallel crystal planes with Miller indices (hkl). When an incident beam of monochromatic X-rays of wavelength λ strikes this set of planes at an angle such that the wave patterns of the beam leaving the various planes are not in phase, no reinforced beam will be produced (Figure 3.25a). Thus, destructive interference occurs. If the reflected wave patterns of the beam leaving the various planes are in phase, then reinforcement of the beam or constructive interference occurs (Fig. 3.25b). 3.11 Crystal Structure Analysis Incident X-rays No reflected X-rays λ d (hkl) planes (a) Incident X-rays Reflected X-rays λ θ θ d (b) Incident X-rays Reflected X-rays Ray 1 Ray 2 (hkl) planes θ θ O M P θ N 2θ d (c) Figure 3.25 The reflection of an X-ray beam by the (hkl) planes of a crystal. (a) No reflected beam is produced at an arbitrary angle of incidence. (b) At the Bragg angle θ, the reflected rays are in phase and reinforce one another. (c) Similar to (b) except that the wave representation has been omitted. (Source: A.G. Guy and J.J. Hren Elements of Physical Metallurgy (3rd ed.). Addison-Wesley, 1974, p. 201.) Let us now consider incident X-rays 1 and 2 as indicated in Figure 3.25c. For these rays to be in phase, the extra distance of travel of ray 2 is equal to MP + PN, which must be an integral number of wavelengths λ. Thus, nλ = MP + PN (3.9) 127 128 CHAPTER 3 Crystal and Amorphous Structure in Materials where n = 1, 2, 3, . . . and is called the order of the diffraction. Since both MP and PN equal dhkl sin θ, where dhkl is the interplanar spacing of the crystal planes of indices (hkl), the condition for constructive interference (i.e., the production of a diffraction peak of intense radiation) must be nλ = 2 dhkl= sin θ (3.10) This equation, known as Bragg’s law,7 gives the relationship among the angular positions of the reinforced diffracted beams in terms of the wavelength λ of the incoming X-ray radiation and of the interplanar spacings dhkl of the crystal planes. In most cases, the first order of diffraction where n = 1 is used, and so for this case, Bragg’s law takes the form λ = 2 dhkl= sin θ (3.11) EXAMPLE PROBLEM 3.15 A sample of BCC iron was placed in an X-ray diffractometer using incoming X-rays with a wavelength λ = 0.1541 nm. Diffraction from the {110} planes was obtained at 2θ = 44.70°. Calculate a value for the lattice constant a of BCC iron. (Assume first-order diffraction with n = 1.) ■ Solution 2θ = 44.704⚬ θ = 22 .35⚬ λ = 2 dhklsin θ λ 0.1541 nm d110 = ______= ____________ 2 sin θ 2(sin 22.35⚬) (3.11) 0.1541 nm = _________ = 0.2026 nm 2(0.3803) Rearranging Eq. 3.5 gives ________ a = dhkl√h2+ k2+ l2 Thus, ___________ (Fe)= d110√12+ 12+ 02 a = (0.2026 nm)(1.414)= 0.2865 nm ◂ 3.11.3 X-Ray Diffraction Analysis of Crystal Structures The Powder Method of X-Ray Diffraction Analysis The most commonly used X-ray diffraction technique is the powder method. In this technique, a powdered specimen is utilized so that there will be a random orientation of many crystals to ensure that some of the particles will be oriented in the X-ray beam to satisfy the diffraction conditions of 7 William Henry Bragg (1862–1942). English physicist who worked on X-ray crystallography. 3.11 Crystal Structure Analysis Figure 3.26 An X-ray diffractometer (with X-radiation shields removed). (Courtesy of Rigaku) Bragg’s law. Modern X-ray crystal analysis uses an X-ray diffractometer that has a radiation counter to detect the angle and intensity of the diffracted beam (Fig. 3.26). A recorder automatically plots the intensity of the diffracted beam as the counter moves on a ­goniometer8 circle (Fig. 3.27) that is in synchronization with the specimen over a range of 2θ values. Figure 3.28 shows an X-ray diffraction recorder chart for the intensity of the diffracted beam versus the diffraction angles 2θ for a powdered pure-metal specimen. In this way, both the angles of the diffracted beams and their intensities can be recorded at one time. Sometimes a powder camera with an enclosed filmstrip is used instead of the diffractometer, but this method is much slower and in most cases, less convenient. Diffraction Conditions for Cubic Unit Cells X-ray diffraction techniques enable the structures of crystalline solids to be determined. The interpretation of X-ray diffraction data for most crystalline substances is complex and beyond the scope of this 8 A goniometer is an instrument for measuring angles. 129 130 CHAPTER 3 Crystal and Amorphous Structure in Materials Radiation detector 120 110 100 Radiation detector (moving on goniometer circle) 90 80 70 60 Diffracted beam 50 2θ Portion of one crystal in specimen 40 30 Plane 1 λ 20 Plane 2 10 0 Incident beam Radiation generator Top view of specimen fixed in goniometer 2θ d θ Radiation generator d sin θ Parallel (hkl) planes in crystal Figure 3.27 Schematic illustration of the diffractometer method of crystal analysis and of the conditions ­necessary for diffraction. Intensity of diffracted beam (cps) (Source: A.G. Guy, Essentials of Materials Science, McGraw-Hill, 1976.) 200 12,000 10,000 8,000 6,000 110 4,000 2,000 0 20 310 211 220 40 60 80 100 Diffraction angle 2θ 400 321 222 120 140 160 Figure 3.28 Record of the diffraction angles for a tungsten sample obtained by the use of a diffractometer with copper radiation. (Source: A.G. Guy and J.J. Hren, Elements of Physical Metallurgy 3rd ed., AddisonWesley, 1974, p. 208.) book, and so only the simple case of diffraction in pure cubic metals will be considered. The analysis of X-ray diffraction data for cubic unit cells can be simplified by combining Eq. 3.4, a dhkl= _________ ________ √h2+ k2+ l2 3.11 Crystal Structure Analysis with the Bragg equation λ = 2d sin θ, giving 2a sin θ λ = _________ ________ √h2+ k2+ l2 (3.12) This equation can be used along with X-ray diffraction data to determine if a cubic crystal structure is body-centered or face-centered cubic. The rest of this subsection will describe how this is done. To use Eq. 3.12 for diffraction analysis, we must know which crystal planes are the diffracting planes for each type of crystal structure. For the simple cubic lattice, reflections from all (hkl) planes are possible. However, for the BCC structure, diffraction occurs only on planes whose Miller indices when added together (h + k + l) total to an even number (Table 3.6). Thus, for the BCC crystal structure, the principal diffracting planes are {110}, {200}, {211}, etc., which are listed in Table 3.7. In the case of the FCC crystal structure, the principal diffracting planes are those whose Miller indices are either all even or all odd (zero is considered even). Thus, for the FCC crystal structure, the diffracting planes are {111}, {200}, {220}, etc., which are listed in Table 3.7. Interpreting Experimental X-Ray Diffraction Data for Metals with Cubic Crystal Structures We can use X-ray diffractometer data to determine crystal structures. A simple case to illustrate how this analysis can be used is to distinguish between the Table 3.6 Rules for determining the diffracting {hkl} planes in cubic crystals Bravais Lattice BCC FCC Reflections Present Reflections Absent (h + k + l) = even (h, k, l) all odd or all even (h + k + l) = odd (h, k, l) not all odd or all even Table 3.7 Miller indices of the diffracting planes for BCC and FCC lattices Cubic Planes {hkl} {100} {110} {111} {200} {210} {211} ... {220} {221} {310} h2 + k2 + l2 12 02 02 + + 12 + 12 + 02 12 + 12 + 12 22 + 02 + 02 22 + 12 + 02 22 + 12 + 12 22 + 22 + 02 22 + 22 + 12 32 + 12 + 02 Sum Σ[h2 + k2 + l2] 1 2 3 4 5 6 7 8 9 10 Cubic Diffracting Planes {hkl} FCC BCC ... 111 200 110 ... 211 220 220 ... 310 200 131 132 CHAPTER 3 Crystal and Amorphous Structure in Materials BCC and FCC crystal structures of a cubic metal. Let us assume that we have a metal with either a BCC or an FCC crystal structure and that we can identify the principal diffracting planes and their corresponding 2θ values, as indicated for the metal tungsten in Figure 3.28. By squaring both sides of Eq. 3.12 and solving for sin2θ, we obtain λ2(h2+ k2+ l2) ____________ sin2θ = 4 a2 (3.13) From X-ray diffraction data, we can obtain experimental values of 2θ for a series of principal diffracting {hkl} planes. Since the wavelength of the incoming radiation and the lattice constant a are both constants, we can eliminate these quantities by forming the ratio of two sin2 θ values as sin2θ h2A+ k2A+ l2A ______ 2 A = _________ sin θB h2B+ k2B+ l2B (3.14) where θA and θB are two diffracting angles associated with the principal diffracting planes {hAkAlA} and {hBkBlB}, respectively. Using Eq. 3.14 and the Miller indices of the first two sets of principal diffracting planes listed in Table 3.7 for BCC and FCC crystal structures, we can determine values for the sin2θ ratios for both BCC and FCC structures. For the BCC crystal structure, the first two sets of principal diffracting planes are the {110} and {200} planes (Table 3.7). Substitution of the Miller {hkl} indices of these planes into Eq. 3.14 gives sin2θ 12+ 12+ 02 ______ 2 A = _________ = 0.5 sin θB 22+ 02+ 02 (3.15) Thus, if the crystal structure of the unknown cubic metal is BCC, the ratio of the sin2θ values that correspond to the first two principal diffracting planes will be 0.5. For the FCC crystal structure, the first two sets of principal diffracting planes are the {111} and {200} planes (Table 3.7). Substitution of the Miller {hkl} indices of these planes into Eq. 3.15 gives sin2θ 12+ 12+ 12 ________ 2 A = _________ = 0.75 sin θB 22+ 02+ 02 (3.16) Thus, if the crystal structure of the unknown cubic metal is FCC, the ratio of the sin2θ values that correspond to the first two principal diffracting planes will be 0.75. Example Problem 3.16 uses Eq. 3.14 and experimental X-ray diffraction data for the 2θ values for the principal diffracting planes to determine whether an unknown cubic metal is BCC or FCC. X-ray diffraction analysis is usually much more complicated than Example Problem 3.16, but the principles used are the same. Both experimental and theoretical X-ray diffraction analysis has been and continues to be used for the determination of the crystal structure of materials. 3.11 Crystal Structure Analysis An X-ray diffractometer recorder chart for an element that has either the BCC or the FCC crystal structure shows diffraction peaks at the following 2θ angles: 40, 58, 73, 86.8, 100.4, and 114.7. The wavelength of the incoming X-ray used was 0.154 nm. a. Determine the cubic structure of the element. b. Determine the lattice constant of the element. c. Identify the element. ■ Solution a. Determination of the crystal structure of the element. First, the sin2 θ values are calculated from the 2θ diffraction angles. 2θ(deg) θ(deg) sin θ sin2 θ 40 58 73 86.8 100.4 114.7 20 29 36.5 43.4 50.2 57.35 0.3420 0.4848 0.5948 0.6871 0.7683 0.8420 0.1170 0.2350 0.3538 0.4721 0.5903 0.7090 Next, the ratio of the sin2θ values of the first and second angles is calculated: 2 sin θ 0.117 _____= _____ = 0.498 ≈ 0.5 sin2θ 0.235 The crystal structure is BCC since this ratio is ≈ 0.5. If the ratio had been ≈ 0.75, the structure would have been FCC. b. Determination of the lattice constant. Rearranging Eq. 3.14 and solving for a2 gives λ2h2+ k2+ l2 a2= __ ________ 4 sin2θ or (3.17) _________ 2√ λ h + k + l a = __ ________ 2 2 2 sin2θ (3.18) Substituting into Eq. 3.18 h = 1, k = 1, and l = 0 for the h, k, l Miller indices of the first set of principal diffracting planes for the BCC crystal structure, which are the {110} planes, the corresponding value for sin2θ, which is 0.117, and 0.154 nm for λ, the incoming radiation, gives _________ √ 0.154 nm _________ 12+ 12+ 02 = ________ a = 0.318 nm ◂ 2 0.117 c. Identification of the element. The element is tungsten since this element has a lattice constant of 0.316 nm and is BCC. 133 EXAMPLE PROBLEM 3.16 134 CHAPTER 3 Crystal and Amorphous Structure in Materials 3.12 AMORPHOUS MATERIALS As discussed previously, some materials are called amorphous or noncrystalline because they lack long-range order in their atomic structure. It should be noted that, in general, materials have a tendency to achieve a crystalline state because that is the most stable state and it corresponds to the lowest energy level. However, atoms in amorphous materials are bonded in a disordered manner because of factors that inhibit the formation of a periodic arrangement. Atoms in amorphous materials, therefore, occupy random spatial positions as opposed to specific positions in crystalline solids. For clarity, various degrees of order (or disorder) are shown in Figure 3.29. Most polymers, glasses, and some metals are members of the amorphous class of materials. In polymers, the secondary bonds among molecules do not allow for the formation of parallel and tightly packed chains during solidification. As a result, polymers such as polyvinylchloride consist of long, twisted molecular chains that are entangled to form a solid with amorphous structure, similar to Figure 3.29c. In some polymers such as polyethylene, the molecules are more efficiently and tightly packed in some regions of the material and produce a higher degree of regional longrange order. As a result, these polymers are often classified as semicrystalline. A more detailed discussion of semicrystalline polymers will be given in Chapter 10. Inorganic glass based on glass-forming oxide, silica (SiO2), is generally characterized as a ceramic material (ceramic glass) and is another example of a material with an amorphous structure. In this type of glass, the fundamental subunit in the molecules is the SiO4− 4 tetrahedron. The ideal crystalline structure of this glass is shown in Figure 3.29a. The schematic shows the Si–O tetrahedrons joined corner to corner to form long-range order. In its viscous liquid state, the molecules have limited mobility, and, in general, crystallization occurs slowly. Therefore, a modest cooling rate suppresses the formation of the crystal structure, and instead the tetrahedra join corner to corner to form a network lacking in long-range order (Fig. 3.29b). In addition to polymers and glasses, some metals also have the ability to form amorphous structures (metallic glass) under strict and often difficult-to-achieve conditions. Unlike glasses, metals have very small and mobile building blocks under molten (a) Figure 3.29 (b) (c) A schematic showing various degrees of order in materials: (a) long-range order in crystalline silica, (b) silica glass without long-range order, and (c) amorphous structure in polymers. 3.13 Summary conditions. As a result, it is difficult to prevent metals from crystallizing. However, alloys such as 78%Fe–9%Si–13%B that contain a high percentage of semimetals, Si and B, may form metallic glasses through rapid solidification at cooling rates in excess of 108 °C/s. At such high cooling rates, the atoms simply do not have enough time to form a crystalline structure and instead form a metal with an amorphous structure, that is, they are highly disordered. In theory, any crystalline material can form a noncrystalline structure if solidified rapidly enough from a molten state. Amorphous materials, because of their structure, possess properties that are superior. For instance, metallic glasses possess higher strength, better corrosion characteristics, and magnetic properties when compared to their crystalline counterparts. Finally, it is important to note that amorphous materials do not show sharp diffraction patterns when analyzed using X-ray diffraction techniques. This is due to a lack of order and periodicity in the atomic structure. In future chapters, the role of structure of the material on its properties will be explained in detail. 3.13 S U M M A R Y Atomic arrangements in crystalline solids can be described by a network of lines called a space lattice. Each space lattice can be described by specifying the atom positions in a repeating unit cell. The crystal structure consists of space lattice and motif or basis. Crystalline materials, such as most metals, possess long-range atomic order. But some materials, such as many polymers and glasses, possess only short-range order. Such materials are called semicrystalline or amorphous. There are seven crystal systems based on the geometry of the axial lengths and interaxial angles of the unit cells. These seven systems have a total of 14 sublattices (unit cells) based on the internal arrangements of atomic sites within the unit cells. In metals, the most common crystal structure unit cells are: body-centered cubic (BCC), face-centered cubic (FCC), and hexagonal close-packed (HCP) (which is a dense variation of the simple hexagonal structure). Crystal directions in cubic crystals are the vector components of the directions resolved along each of the component axes and reduced to smallest integers. They are indicated as [uvw]. Families of directions are indexed by the direction indices enclosed by pointed brackets as ⟨uvw⟩. Crystal planes in cubic crystals are indexed by the reciprocals of the axial intercepts of the plane (followed by the elimination of fractions) as (hkl). Cubic crystal planes of a form (family) are indexed with braces as {hkl}. Crystal planes in hexagonal crystals are commonly indexed by four indices h, k, i, and l enclosed in parentheses as (hkil). These indices are the reciprocals of the intercepts of the plane on the a1, a2, a3, and c axes of the hexagonal crystal structure unit cell. Crystal directions in hexagonal crystals are the vector components of the direction resolved along each of the four coordinate axes and reduced to smallest integers as [uvtw]. Using the hard-sphere model for atoms, calculations can be made for the volume, planar, and linear density of atoms in unit cells. Planes in which atoms are packed as tightly as possible are called close-packed planes, and directions in which atoms are in closest contact are called close-packed directions. Atomic packing factors for different crystal structures can also be determined by assuming the hard-sphere atomic model. Some metals have different crystal structures at different ranges of temperature and pressure, a phenomenon called polymorphism. 135 136 CHAPTER 3 Crystal and Amorphous Structure in Materials Crystal structures of crystalline solids can be determined by using X-ray diffraction analysis techniques. X-rays are diffracted in crystals when the Bragg’s law (nλ = 2d sin θ) conditions are satisfied. By using the X-ray diffractometer and the powder method, the crystal structure of many crystalline solids can be determined. 3.14 DEFINITIONS Sec. 3.1 Amorphous: lacking in long-range atomic order. Crystal: a solid composed of atoms, ions, or molecules arranged in a pattern that is repeated in three dimensions. Crystal structure: a regular three-dimensional pattern of atoms or ions in space. Space lattice: a three-dimensional array of points each of which has identical surroundings. Lattice point: one point in an array in which all the points have identical surroundings. Unit cell: a convenient repeating unit of a space lattice. The axial lengths and axial angles are the lattice constants of the unit cell. Motif (or Basis): a group of atoms that are organized relative to each other and are associated with corresponding lattice points. Sec. 3.3 Body-centered cubic (BCC) unit cell: a unit cell with an atomic packing arrangement in which one atom is in contact with eight identical atoms located at the corners of an imaginary cube. Face-centered cubic (FCC) unit cell: a unit cell with an atomic packing arrangement in which 12 atoms surround a central atom. The stacking sequence of layers of close-packed planes in the FCC crystal structure is ABCABC. . . . Hexagonal close-packed (HCP) unit cell: a unit cell with an atomic packing arrangement in which 12 atoms surround a central identical atom. The stacking sequence of layers of close-packed planes in the HCP crystal structure is ABABAB.... Atomic packing factor (APF): the volume of atoms in a selected unit cell divided by the volume of the unit cell. Sec. 3.5 Indices of direction in a cubic crystal: a direction in a cubic unit cell is indicated by a vector drawn from the origin at one point in a unit cell through the surface of the unit cell; the position coordinates (x, y, and z) of the vector where it leaves the surface of the unit cell (with fractions cleared) are the indices of direction. These indices, designated u, v, and w, are enclosed in brackets as [uvw]. Negative indices are indicated by a bar over the index. Sec. 3.6 Indices for cubic crystal planes (Miller indices): the reciprocals of the intercepts (with fractions cleared) of a crystal plane with the x, y, and z axes of a unit cube are called the Miller indices of that plane. They are designated h, k, and l for the x, y, and z axes, respectively, and are enclosed in parentheses as (hkl). Note that the selected crystal plane must not pass through the origin of the x, y, and z axes. Sec. 3.9 Volume density ρv: mass per unit volume; this quantity is usually expressed in Mg/m3 or g/cm3. 3.15 Problems Planar density ρp: the equivalent number of atoms whose centers are intersected by a selected area divided by the selected area. Linear density ρl: the number of atoms whose centers lie on a specific direction on a specific length of line in a unit cube. Repeat Distance: The distance between two consecutive lattice points along a specific direction. Sec. 3.10 Polymorphism (as pertains to metals): the ability of a metal to exist in two or more crystal structures. For example, iron can have a BCC or an FCC crystal structure, depending on the temperature. Sec. 3.12 Semicrystalline: materials with regions of crystalline structure dispersed in the surrounding, amorphous region, for instance, some polymers. Metallic glass: metals with an amorphous atomic structure. 3.15 PROBLEMS Answers to problems marked with an asterisk are given at the end of the book. Knowledge and Comprehension Problems 3.1 Define the following terms: (a) crystalline solid, (b) long-range order, (c) short-range order, and (d) amorphous. 3.2 Define the following terms: (a) crystal structure, (b) space lattice, (c) lattice point, (d) unit cell, (e) motif, and (f) lattice constants. 3.3 What are the 14 Bravais unit cells? 3.4 What are the three most common metal crystal structures? List five metals that have each of these crystal structures. 3.5 For a BCC unit cell, (a) how many atoms are there inside the unit cell, (b) what is the coordination number for the atoms, (c) what is the relationship between the length of the side a of the BCC unit cell and the radius of its atoms, and (d) what is the atomic packing factor? 3.6 For an FCC unit cell, (a) how many atoms are there inside the unit cell, (b) what is the coordination number for the atoms, (c) what is the relationship between the length of the side a of the FCC unit cell and the radius of its atoms, and (d) what is the atomic packing factor? 3.7 For an HCP unit cell (consider the primitive cell), (a) how many atoms are there inside the unit cell, (b) what is the coordination number for the atoms, (c) what is the atomic packing factor, (d) what is the ideal c/a ratio for HCP metals, and (e) repeat (a) through (c) considering the “larger” cell. 3.8 How are atomic positions located in cubic unit cells? 3.9 List the atom positions for the eight corner and six face-centered atoms of the FCC unit cell. 3.10 How are the indices for a crystallographic direction in a cubic unit cell determined? 137 138 CHAPTER 3 Tutorial Crystal and Amorphous Structure in Materials 3.11 What are the crystallographic directions of a family or form? What generalized notation is used to indicate them? 3.12 How are the Miller indices for a crystallographic plane in a cubic unit cell determined? What generalized notation is used to indicate them? 3.13 What is the notation used to indicate a family or form of cubic crystallographic planes? 3.14 How are crystallographic planes indicated in HCP unit cells? 3.15 What notation is used to describe HCP crystal planes? 3.16 What is the difference in the stacking arrangement of close-packed planes in (a) the HCP crystal structure and (b) the FCC crystal structure? 3.17 What are the closest-packed directions in (a) the BCC structure, (b) the FCC structure, and (c) the HCP structure? 3.18 Identify the close-packed planes in (a) the BCC structure, (b) the FCC structure, and (c) the HCP structure. 3.19 What is polymorphism with respect to metals? 3.20 What are X-rays, and how are they produced? 3.21 Draw a schematic diagram of an X-ray tube used for X-ray diffraction, and indicate on it the path of the electrons and X-rays. 3.22 What is the characteristic X-ray radiation? What is its origin? 3.23 Distinguish between destructive interference and constructive interference of reflected X-ray beams through crystals. Application and Analysis Problems 3.24 Tungsten at 20°C is BCC and has an atomic radius of 0.137 nm. (a) Calculate a value for its lattice constant a in nanometers. (b) Calculate the volume of the unit cell. 3.25 Lead is FCC and has an atomic radius of 0.175 nm. (a) Calculate a value for its lattice constant a in nanometers. (b) Calculate the volume of the unit cell in nm3. 3.26 Verify that the atomic packing factor for the FCC structure is 0.74. 3.27 Calculate the volume in cubic nanometers of the cobalt crystal structure unit cell (use the larger cell). Cobalt is HCP at 20°C with a = 0.2507 nm and c = 0.4069 nm. 3.28 Consider a 0.05-mm-thick, 500 mm2 (about three times the area of a dime) piece of aluminum foil. How many unit cells exist in the foil? If the density of aluminum is 2.7 g/cm3, what is the mass of each cell? 3.29 Draw the following directions in a BCC unit cell, and list the position coordinates of the atoms whose centers are intersected by the direction vector. Determine the repeat distance in terms of the lattice constant in each direction. (a) [010] (b) [011] (c) [111] (d) Find the angle between directions in (b) and (c). 3.30 Draw direction vectors in an FCC unit cell for the following cubic directions, and list the position coordinates of the atoms whose centers are intersected by the direction vector. Determine the repeat distance in terms of the lattice constant in each direction. ¯ ¯ (a) [ ¯ 1 1] (b) [ 1 10¯ 1] (c) [2¯ ¯ 1 ] (d) [ 1 3¯ 1 ] 1 (e) Find the angle between directions in (b) and (d). 3.15 Problems 139 z z a 1 4 1 3 h c 3 4 b 1 2 1 2 1 3 e d 2 3 1 4 3 4 f g 1 4 1 2 x y 1 4 y 3 4 x (a) (b) Figure P3.32 3.31 Draw direction vectors in unit cells for the following cubic directions: ¯ (a) [ 1¯ ¯ 1 ] (b) [ 2 1¯ 3] (c) [ 2 31] (d) [ 3 0¯ 1] (e) [ 2 2¯ 2] (f) [ 1 2¯ 3] 3 ¯ ¯ ¯ ¯ ¯ ¯ (g) [ 01] (h) [ 1 121] (i) [321] (j) [ 103] (k) [ 12 2 ] (l) [ ¯ 2 3] 2 3.32 What are the indices of the directions shown in the unit cubes of Figure P3.32? 3.33 A direction vector passes through a unit cube from the ( _34 , 0, _ 14 ) to the ( _12 , 1, 0) ­positions. What are its direction indices? 3.34 A direction vector passes through a unit cube from the (1, 0, _ 34 ) to the ( _41 , 1, _ 14 ) ­positions. What are its direction indices? 3.35 What are the directions of the ⟨10¯ 3⟩ family or form for a unit cube? Draw all ­directions in a unit cell. 3.36 What are the directions of the ⟨111⟩ family or form for a unit cube? Draw all ­directions in a BCC unit cell. Can you identify a special quality of these directions? 3.37 What ⟨110⟩ type directions lie on the (111) plane of a cubic unit cell? Draw those directions in an FCC unit cell. Can you identify a special quality of these directions? 3.38 What ⟨111⟩ type directions lie on the (110) plane of a BCC unit cell? Draw those directions in a unit cell. Can you identify a special quality of these directions? 3.39 Draw in unit cubes the crystal planes that have the following Miller indices: (a) ( 1¯ ¯ 1 ) (b) ( 1 10¯ 2) (c) ( 1¯ ¯ 2 ) (d) ( 1 21¯ 3) (e) ( 3¯ 1) (f) ( 2 30¯ 2) ¯ ¯ ¯ ¯ ¯ ¯ ¯ (g) ( 201) (h) ( 12 2 ) (i) ( 32) (j) ( 2 133) (k) ( 31 2) (l) ( 3¯ 3 ) 1 3.40 What are the Miller indices of the cubic crystallographic planes shown in Figure P3.40? 3.41 What are the {100} family of planes of the cubic system? Draw those planes in a BCC unit cell and show all atoms whose centers are intersected by the planes. What is your conclusion? 3.42 Draw the following crystallographic planes in a BCC unit cell, and list the position of the atoms whose centers are intersected by each of the planes: (a) (010) (b) (011) (c) (111) Confirming Pages 140 CHAPTER 3 z z 2 3 3 4 1 4 3 4 a 1 3 Crystal and Amorphous Structure in Materials b a b 1 3 d 1 2 1 3 2 3 d c y c 1 3 x (a) y x 2 3 (b) Figure P3.40 Tutorial smi96553_ch03_092-145.indd 140 3.43 Draw the following crystallographic planes in an FCC unit cell, and list the position coordinates of the atoms whose centers are intersected by each of the planes: (a) (010) (b) (011) (c) (111) 3.44 A cubic plane has the following axial intercepts: a = _ 13 , b = − _ 23 , c = _ 12 . What are the Miller indices of this plane? 3.45 A cubic plane has the following axial intercepts: a = − _ 12 , b = − _ 12 , c = _ 23 . What are the Miller indices of this plane? 3.46 Determine the Miller indices of the cubic crystal plane that intersects the following position coordinates: ( 1, _ 12 , 1); ( _12 , 0, _ 34 ); (1, 0, _ 12 ). 3.47 Determine the Miller indices of the cubic crystal plane that intersects the following position coordinates: ( 0, 0, _ 12 ); (1, 0, 0); ( _12 , _ 14 , 0). 3.48 Rodium is FCC and has a lattice constant a of 0.38044 nm. Calculate the following interplanar spacings: (a) d111 (b) d200 (c) d220 3.49 Tungsten is BCC and has a lattice constant a of 0.31648 nm. Calculate the following interplanar spacings: (a) d110 (b) d220 (c) d310 3.50 The d310 interplanar spacing in a BCC element is 0.1587 nm. (a) What is its ­lattice constant a? (b) What is the atomic radius of the element? (c) What could this element be? 3.51 The d422 interplanar spacing in an FCC metal is 0.083397 nm. (a) What is its lattice constant a? (b) What is the atomic radius of the metal? (c) What could this metal be? 3.52 Draw the hexagonal crystal planes whose Miller-Bravais indices are: ¯ (a) ( 10¯ 11) (b) ( 01¯ 11) (c) ( 2¯ 1 0) (d) ( 1 1¯ 12) (e) ( 2 2¯ 1¯ 1) (f) ( 1 1¯ 01) 1 ¯ ¯ ¯ ¯ (g) ( 2¯ 1 2) (h) ( 1 2¯ 200) (i) ( 10¯ 12) (j) ( 100) (k) ( 1 111) (l) ( 2 012) 1 3.53 Determine the Miller-Bravais indices of the hexagonal crystal planes in Figure P3.53. 07/02/18 10:08 AM 3.15 Problems b a3 a3 a c 1 2 -a1 -a1 a c -a2 a2 b -a2 -a3 a1 a2 -a3 a1 (a) (b) Figure P3.53 3.54 Determine the Miller-Bravais direction indices of the −a1, −a2, and −a3 directions. 3.55 Determine the Miller-Bravais direction indices of the vectors originating at the center of the lower basal plane and ending at the endpoints of the upper basal plane as indicated in Figure 3.16d. 3.56 Determine the Miller-Bravais direction indices of the basal plane of the vectors originating at the center of the lower basal plane and exiting at the midpoints between the principal planar axes. 3.57 Determine the Miller-Bravais direction indices of the directions indicated in Figure P3.57. 3.58 The lattice constant for BCC tantalum at 20°C is 0.33026 nm and its density is 16.6 g/cm3. Calculate a value for its relative atomic mass. 3.59 Calculate a value for the density of FCC platinum in grams per cubic centimeter from its lattice constant a of 0.39239 nm and its atomic mass of 195.09 g/mol. a2 -a1 -a3 a3 -a2 a1 (a) Figure P3.57 a2 -a1 -a3 a3 -a2 a1 (b) 141 142 CHAPTER 3 Crystal and Amorphous Structure in Materials 3.60 Calculate the planar atomic density in atoms per square millimeter for the following crystal planes in BCC chromium, which has a lattice constant of 0.28846 nm. Compare the values and draw a conclusion. (a) (100), (b) (110), (c) (111). 3.61 Calculate the planar atomic density in atoms per square millimeter for the following crystal planes in FCC gold, which has a lattice constant of 0.40788 nm. Compare the values and draw a conclusion. (a) (100), (b) (110), (c) (111). 3.62 Calculate the planar atomic density in atoms per square millimeter for the (0001) plane in HCP beryllium, which has a lattice constant a = 0.22856 nm and a c constant of 0.35832 nm. Can you make any observations about this plane? 3.63 Calculate the linear atomic density in atoms per millimeter for the following ­directions in BCC vanadium, which has a lattice constant of 0.3039 nm: (a) [100], (b) [110], (c) [111]. Determine the repeat distance along each direction. 3.64 Calculate the linear atomic density in atoms per millimeter for the following directions in FCC iridium, which has a lattice constant of 0.38389 nm: (a) [100], (b) [110], (c) [111]. Determine the repeat distance along each direction. 3.65 Titanium goes through a polymorphic change from BCC to HCP crystal structure upon cooling through 332°C. Calculate the percentage change in volume when the crystal structure changes from BCC to HCP. The lattice constant a of the BCC unit cell at 882°C is 0.332 nm, and the HCP unit cell has a = 0.2950 nm and c = 0.4683 nm. 3.66 Pure iron goes through a polymorphic change from BCC to FCC upon heating through 912°C. Calculate the volume change associated with the change in crystal structure from BCC to FCC if at 912°C the BCC unit cell has a lattice constant a = 0.293 nm and the FCC unit cell a = 0.363 nm. 3.67 Derive Bragg’s law by using the simple case of incident X-ray beams being diffracted by parallel planes in a crystal. 3.68 A sample of BCC metal was placed in an X-ray diffractometer using X-rays with a wavelength of λ = 0.1541 nm. Diffraction from the {221} planes was obtained at 2θ = 88.838°. Calculate a value for the lattice constant a for this BCC elemental metal. (Assume first-order diffraction, n = 1.) 3.69 X-rays of an unknown wavelength are diffracted by a gold sample. The 2θ angle was 64.582° for the {220} planes. What is the wavelength of the X-rays used? (The lattice constant of gold = 0.40788 nm; assume first-order diffraction, n = 1.) 3.70 An X-ray diffractometer recorder chart for an element that has either the BCC or the FCC crystal structure showed diffraction peaks at the following 2θ angles: 41.069°, 47.782°, 69.879°, and 84.396°. The wavelength of the incoming radiation was 0.15405 nm. (X-ray diffraction data courtesy of the International Centre for Diffraction Data.) (a) Determine the crystal structure of the element. (b) Determine the lattice constant of the element. (c) Identify the element. 3.71 An X-ray diffractometer recorder chart for an element that has either the BCC or the FCC crystal structure showed diffraction peaks at the following 2θ angles: 38.60°, 55.71°, 69.70°, 82.55°, 95.00°, and 107.67°. Wavelength λ of the incoming radiation was 0.15405 nm. (a) Determine the crystal structure of the element. (b) Determine the lattice constant of the element. (c) Identify the element. 3.15 Problems 3.72 An X-ray diffractometer recorder chart for an element that has either the BCC or the FCC crystal structure showed diffraction peaks at the following 2θ angles: 36.191°, 51.974°, 64.982°, and 76.663°. The wavelength of the incoming radiation was 0.15405 nm. (a) Determine the crystal structure of the element. (b) Determine the lattice constant of the element. (c) Identify the element. 3.73 An X-ray diffractometer recorder chart for an element that has either the BCC or the FCC crystal structure showed diffraction peaks at the following 2θ angles: 40.663°, 47.314°, 69.144°, and 83.448°. Wavelength l of the incoming radiation was 0.15405 nm. (a) Determine the crystal structure of the element. (b) Determine the lattice constant of the element. (c) Identify the element. Synthesis and Evaluation Problems 3.74 Do you expect iron and silver to have the same (a) atomic packing factor, (b) volume of unit cell, (c) number of atoms per unit cell, and (d) coordination number? How about gold and silver? How about titanium and silver? 3.75 In a cubic unit cell, draw the (111) and (011) planes. Highlight the intersection of the two planes. What are the direction indices of the intersection line? 3.76 In a cubic unit cell, draw the (011) and (110) planes. Highlight the intersection of the two planes. What are the direction indices of the intersection line? 3.77 Show using geometry that the ideal c/a ratio of the hexagonal close-packed unit cell (when atoms are perfect spheres) is 1.633. Hint: Draw the center atom in the top basal plane in contact with the three atoms in the center of the HCP cell; connect the centers of the three atoms inside the HCP cell to each other and to the atom at the center of one of the basal planes. 3.78 Assuming that the volume of an HCP metal cell (larger cell) is 0.09130 nm3 and the c/a ratio is 1.856, determine (a) the values for c and a, and (b) the radius, R, of the atom. (c) If you were told that the metal is zinc, would you be surprised? How do you explain the discrepancy? 3.79 Assuming that the volume of an HCP metal cell (larger cell) is 0.01060 nm3 and the c/a ratio is 1.587, determine (a) the values for c and a, and (b) the radius, R, of the atom. (c) If you were told that the metal is titanium, does the calculated R match that of Ti? How do you explain the discrepancy? 3.80 The structure of NaCl (an ionic material) is given in Figure 2.18b. Determine (a) its lattice constant a, and (b) its density. Hint: Since NaCl is ionic, use the ion radius data and note the atomic radii. 3.81 The unit cell structure of the ionic solid, CsI, is similar to that in Figure 2.18a. Determine (a) its packing factor, and (b) compare this packing factor with that of BCC metals. Explain the difference, if any. 3.82 Iron (below 912°C) and tungsten are both BCC with significantly different atomic radii. However, they have the same atomic packing factor of 0.68. How do you explain this? 3.83 Verify that there are eight atoms inside a diamond cubic structure (see Figure 2.23b and c). Draw a 3D schematic of the atoms inside the cell. 143 144 CHAPTER 3 Crystal and Amorphous Structure in Materials 3.84 The lattice constant for the diamond cubic structure of diamond is 0.357 nm. Diamond is metastable, meaning that it will transform to graphite at elevated temperatures. If this transformation occurs, what percent volume change will occur? (Density of graphite is 2.25 gr/cm3) 3.85 Calculate the center-to-center distance between adjacent atoms of gold along the following directions: (a) [100], (b) [101], (c) [111], and (d) [102]. Speculate as to why such information may be important in understanding the behavior of the material. 3.86 Calculate the center-to-center distance between adjacent atoms of tungsten along the following directions: (a) [100], (b) [101], (c) [111], and (d) [102]. Speculate as to why such information may be important in understanding the behavior of the material. 3.87 A plane in a cubic crystal intersects the x axis at 0.25, the y axis at 2, and is parallel to the z axis. What are the Miller indices for this plane? Draw this plane in a single cube and show all key dimensions. 3.88 A plane in a cubic crystal intersects the x axis at 3, the y axis at 1, and the z axis at 1. What are the Miller indices for this plane? Draw this plane in a single cube and show all key dimensions. 3.89 A plane in a hexagonal crystal intersects at the a1 axis at −1, the a2 axis at 1, and the c axis at infinity. What are the Miller indices for this plane? Draw this plane in a hexagonal unit cell and show all key dimensions. 3.90 A plane in a hexagonal crystal intersects at the a1 axis at 1, the a2 axis at 1, and the c axis at 0.5. What are the Miller indices for this plane? Draw this plane in a hexagonal unit cell and show all key dimensions. 3.91 Without drawing any of the hexagonal planes given below, determine which of the planes is, in fact, not a plane. (a) (¯ 0¯ 1 0), (b) (10¯ 1 10), and (c) (¯ 1¯ 1 0). 1 3.92 Name as many carbon allotropes as you can, and discuss their crystal structure. 3.93 A thin layer of aluminum nitride is sometimes deposited on silicon wafers at high temperatures (1000°C). The coefficient of thermal expansion and the lattice constant of the silicon crystal is different than that of aluminum nitride. Will this cause a problem? Explain. 3.94 An unknown material is being analyzed using X-ray diffraction techniques. However, the diffraction patterns are extremely broad (no clear peaks are visible). (a) What does this tell you about the material? (b) What are some of the tests that you can perform to help identify the material or narrow the possibilities? 3.95 Explain, in general terms, why many polymers and some ceramic glasses have an amorphous or semicrystalline structure. 3.96 Explain how ultra-rapid cooling of some metal alloys produces metallic glass. 4 C H A P T E R Solidification and Crystalline Imperfections (Courtesy of Stan David and Lynn Boatner, Oak Ridge National Library) W hen molten alloys are cast, solidification starts at the walls of the mold as it is being cooled. The solidification of an alloy (as opposed to a pure metal) takes place not at a specific temperature but over a range of temperatures. While the alloy is in this range, it has a pasty form that consists of solid, treelike structures called dendrites (meaning treelike), and liquid metal. The size and shape of the dendrite depends on the cooling rate. The liquid metal existing among these three-dimensional dendritic structures eventually solidifies to form a completely solid structure that we refer to as the grain structure. The study of dendrites is important because they influence compositional variations, porosity, and segregation and therefore the properties of the cast metal. The figure shows the three-dimensional structure of dendrites. The figure shows a “forest” of dendrites formed during the solidification of a nickel-based superalloy.1 ■ 1 146 http://mgnews.msfc.nasa.gov/IDGE/IDGE.html